data_fuka32
 
_audit_creation_method            SHELXL-97
_chemical_name_systematic
;
 ?
;
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          'C2 H4 Ca8 O22 Si4'
_chemical_formula_sum
 'C2 H4 Ca8 O22 Si4'
_chemical_formula_weight          813.05
 
loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'C'  'C'   0.0181   0.0091
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0492   0.0322
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.2541   0.3302
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.3641   1.2855
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_symmetry_cell_setting            monoclinic
_symmetry_space_group_name_H-M    P21/c
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x, y+1/2, -z+1/2'
 '-x, -y, -z'
 'x, -y-1/2, z-1/2'
 
_cell_length_a                    7.573(3)
_cell_length_b                    23.364(4)
_cell_length_c                    11.544(5)
_cell_angle_alpha                 90.00
_cell_angle_beta                  109.150(10)
_cell_angle_gamma                 90.00
_cell_volume                      1929.5(12)
_cell_formula_units_Z             4
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     25
_cell_measurement_theta_min       20
_cell_measurement_theta_max       25
 
_exptl_crystal_description        plate
_exptl_crystal_colour             colourless
_exptl_crystal_size_max           0.15
_exptl_crystal_size_mid           0.10
_exptl_crystal_size_min           0.05
_exptl_crystal_density_meas       'not measured'
_exptl_crystal_density_diffrn     2.799
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000              1632
_exptl_absorpt_coefficient_mu     7.353
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_correction_T_min   0.332     0.692    
_exptl_absorpt_correction_T_max   0.692    
_exptl_absorpt_process_details    'program MULABS (Blessing R.H., 1995)'
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      1.00000
_diffrn_radiation_type            synchrotron
_diffrn_radiation_source          'fine-focus sealed tube'
_diffrn_radiation_monochromator   graphite
_diffrn_measurement_device_type   'Mar CCD plate'
_diffrn_measurement_method        'integration of the spots (Denzo program)'
_diffrn_detector_area_resol_mean  ?
_diffrn_standards_number          ?
_diffrn_standards_interval_count  ?
_diffrn_standards_interval_time   ?
_diffrn_standards_decay_%         ?
_diffrn_reflns_number             7004
_diffrn_reflns_av_R_equivalents   0.0214
_diffrn_reflns_av_sigmaI/netI     0.0178
_diffrn_reflns_limit_h_min        -7
_diffrn_reflns_limit_h_max        7
_diffrn_reflns_limit_k_min        -23
_diffrn_reflns_limit_k_max        21
_diffrn_reflns_limit_l_min        -11
_diffrn_reflns_limit_l_max        11
_diffrn_reflns_theta_min          2.45
_diffrn_reflns_theta_max          30.01
_reflns_number_total              1958
_reflns_number_gt                 1848
_reflns_threshold_expression      >2sigma(I)
 
_computing_data_collection        ?
_computing_cell_refinement        ?
_computing_data_reduction         'Scalepack (Otwinowski & Minor, 1997)'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1997)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
 
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
 'calc w=1/[σ²(Fo²)+(0.0629P)²+2.1891P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    geom
_refine_ls_hydrogen_treatment     none
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        ?
_refine_ls_number_reflns          1958
_refine_ls_number_parameters      206
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0352
_refine_ls_R_factor_gt            0.0342
_refine_ls_wR_factor_ref          0.1022
_refine_ls_wR_factor_gt           0.1005
_refine_ls_goodness_of_fit_ref    1.111
_refine_ls_restrained_S_all       1.111
_refine_ls_shift/su_max           0.002
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_symmetry_multiplicity
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ca1 Ca 0.43393(14) 0.04361(4) 0.12465(7) 0.0122(3) Uani 1 1 d . . .
Ca1A Ca 0.93909(14) 0.04370(4) 0.12368(7) 0.0115(3) Uani 1 1 d . . .
Ca4 Ca 0.31111(13) -0.04516(4) 0.37343(6) 0.0120(3) Uani 1 1 d . . .
Ca4A Ca 0.81117(13) -0.04573(4) 0.37372(6) 0.0125(3) Uani 1 1 d . . .
Ca2 Ca 0.27677(15) -0.30939(3) 0.30368(7) 0.0147(3) Uani 1 1 d . . .
Ca2A Ca 0.77763(15) -0.30906(3) 0.30742(7) 0.0136(3) Uani 1 1 d . . .
Ca3 Ca 0.59574(15) -0.19320(3) 0.43980(7) 0.0135(3) Uani 1 1 d . . .
Ca3A Ca 0.09625(15) -0.19293(3) 0.44354(7) 0.0144(3) Uani 1 1 d . . .
Si1 Si 0.47434(18) -0.08604(5) 0.12374(10) 0.0145(4) Uani 1 1 d . . .
Si1A Si 0.89978(18) -0.08634(5) 0.12572(10) 0.0142(4) Uani 1 1 d . . .
Si2 Si 0.39457(17) -0.21792(5) 0.12182(10) 0.0152(4) Uani 1 1 d . . .
Si2A Si 0.97984(17) -0.21820(5) 0.12744(9) 0.0152(4) Uani 1 1 d . . .
C1 C 0.3117(6) 0.08155(19) 0.3764(3) 0.0104(11) Uiso 1 1 d . . .
C1A C 0.8149(6) 0.0796(2) 0.3761(3) 0.0109(11) Uiso 1 1 d . . .
O1 O 0.1192(5) 0.05059(11) -0.0049(3) 0.0137(7) Uiso 1 1 d . . .
O1A O 0.6267(5) 0.04888(11) -0.0037(3) 0.0129(7) Uiso 1 1 d . . .
O2 O 0.4915(5) -0.04796(11) 0.2429(2) 0.0128(7) Uiso 1 1 d . . .
O2A O 0.0014(5) -0.04727(11) 0.2436(2) 0.0125(7) Uiso 1 1 d . . .
O3 O 0.3657(6) 0.05147(11) 0.4774(3) 0.0163(7) Uiso 1 1 d . . .
O3A O 0.8632(6) 0.04963(11) 0.4773(3) 0.0158(7) Uiso 1 1 d . . .
O4 O 0.2616(6) 0.05384(12) 0.2740(3) 0.0166(7) Uiso 1 1 d . . .
O4A O 0.7608(6) 0.05181(12) 0.2735(3) 0.0161(7) Uiso 1 1 d . . .
O5 O 0.3164(4) 0.13528(14) 0.3792(2) 0.0200(8) Uiso 1 1 d . . .
O5A O 0.8143(4) 0.13323(14) 0.3786(2) 0.0207(8) Uiso 1 1 d . . .
O6 O 0.5335(4) -0.24214(12) 0.2457(2) 0.0186(7) Uiso 1 1 d . . .
O6A O -0.0246(4) -0.24319(12) 0.2542(2) 0.0185(7) Uiso 1 1 d . . .
O7 O 0.3967(4) -0.24127(11) -0.0067(2) 0.0187(7) Uiso 1 1 d . . .
O7A O 0.8411(4) -0.24085(11) 0.0017(2) 0.0186(7) Uiso 1 1 d . . .
O8 O 0.1865(4) -0.24136(13) 0.12456(19) 0.0185(8) Uiso 1 1 d . . .
O8A O 0.6880(4) -0.10114(13) 0.1275(2) 0.0212(8) Uiso 1 1 d . . .
O9 O 0.3808(4) -0.14786(12) 0.1236(2) 0.0203(8) Uiso 1 1 d . . .
O9A O 0.9952(4) -0.14819(13) 0.1311(3) 0.0201(8) Uiso 1 1 d . . .
OH1 O 0.3091(4) -0.14433(13) 0.3736(2) 0.0126(8) Uiso 1 1 d . . .
OH1A O 0.8174(4) -0.14367(14) 0.3784(2) 0.0126(8) Uiso 1 1 d . . .
OH2 O 0.4434(4) 0.14234(13) 0.1298(2) 0.0128(8) Uiso 1 1 d . . .
OH2A O 0.9347(4) 0.14343(13) 0.1242(2) 0.0136(8) Uiso 1 1 d . . .
H1 H 0.2763 -0.1503 0.2997 0.050 Uiso 1 1 d . . .
H1A H 0.7735 -0.1509 0.2973 0.050 Uiso 1 1 d . . .
H2 H 0.3970 0.1509 0.0516 0.050 Uiso 1 1 d . . .
H2A H 0.8984 0.1479 0.0450 0.050 Uiso 1 1 d . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ca1 OH2 2.308(3) . ?
Ca1 O1 2.367(4) . ?
Ca1 O1A 2.400(4) . ?
Ca1 O4 2.492(4) . ?
Ca1 O2 2.498(3) . ?
Ca1 O4A 2.515(4) . ?
Ca1 O1A 2.531(3) 3_655 ?
Ca1 Si1 3.0448(16) . ?
Ca1 O8A 3.061(3) 3_655 ?
Ca1 Si1A 3.3083(18) 3_655 ?
Ca1 Si1 3.3157(18) 3_655 ?
Ca1 Ca1A 3.744(2) 1_455 ?
Ca1 H2 2.6303 . ?
Ca1A O1 2.328(4) 1_655 ?
Ca1A OH2A 2.330(3) . ?
Ca1A O1A 2.344(4) . ?
Ca1A O2A 2.496(3) 1_655 ?
Ca1A O4 2.501(4) 1_655 ?
Ca1A O4A 2.526(4) . ?
Ca1A O1 2.556(3) 3_655 ?
Ca1A Si1A 3.0537(16) . ?
Ca1A Si1 3.6155(18) 3_655 ?
Ca1A Si1A 3.6160(18) 3_755 ?
Ca1A Ca1 3.744(2) 1_655 ?
Ca1A H2A 2.5813 . ?
Ca4 OH1 2.317(3) . ?
Ca4 O2A 2.333(4) . ?
Ca4 O2 2.343(4) . ?
Ca4 O3A 2.493(4) 3_656 ?
Ca4 O3 2.492(4) 3_656 ?
Ca4 O3 2.526(3) . ?
Ca4 O4 2.554(3) . ?
Ca4 C1 2.961(5) . ?
Ca4 Si1A 3.6003(17) 1_455 ?
Ca4 Si1 3.6175(19) . ?
Ca4 Ca4A 3.7859(18) . ?
Ca4 Ca4A 3.7872(18) 1_455 ?
Ca4 H1 2.5848 . ?
Ca4A OH1A 2.289(3) . ?
Ca4A O2 2.397(4) . ?
Ca4A O2A 2.398(4) 1_655 ?
Ca4A O3A 2.498(3) . ?
Ca4A O3A 2.503(4) 3_756 ?
Ca4A O3 2.505(4) 3_656 ?
Ca4A O4A 2.527(3) . ?
Ca4A C1A 2.930(5) . ?
Ca4A O8A 2.981(3) . ?
Ca4A Si1A 3.2873(18) . ?
Ca4A Si1 3.3002(17) . ?
Ca4A H1A 2.5946 . ?
Ca2 OH2 2.299(3) 2_645 ?
Ca2 OH2A 2.312(3) 2_645 ?
Ca2 O7 2.390(3) 4_556 ?
Ca2 O5A 2.397(3) 2_645 ?
Ca2 O8 2.518(3) . ?
Ca2 O6A 2.659(3) . ?
Ca2 O6 2.748(3) . ?
Ca2 Si2A 3.2762(16) 1_455 ?
Ca2 Si2 3.3164(16) . ?
Ca2 O4A 3.351(3) 2_645 ?
Ca2 Si2 3.541(2) 4_556 ?
Ca2 Ca3 3.6309(15) . ?
Ca2A OH2 2.326(3) 2_645 ?
Ca2A OH2A 2.340(3) 2_745 ?
Ca2A O6 2.347(3) . ?
Ca2A O6A 2.365(3) 1_655 ?
Ca2A O5 2.415(3) 2_645 ?
Ca2A O7A 2.431(3) 4_556 ?
Ca2A O4 3.324(3) 2_645 ?
Ca2A Si2A 3.5618(19) 4_556 ?
Ca2A Ca3 3.5974(16) . ?
Ca2A Ca3A 3.6285(15) 1_655 ?
Ca2A O9A 3.692(3) 4_556 ?
Ca3 OH1A 2.332(3) . ?
Ca3 O7A 2.338(3) 4_556 ?
Ca3 OH1 2.348(3) . ?
Ca3 O7 2.368(3) 4_556 ?
Ca3 O5 2.393(3) 3_656 ?
Ca3 O6 2.420(3) . ?
Ca3 O3 3.432(3) 3_656 ?
Ca3 Si2 3.5298(19) . ?
Ca3 Si2 3.6261(17) 4_556 ?
Ca3 O9 3.633(3) . ?
Ca3 H1 2.6278 . ?
Ca3 H1A 2.6358 . ?
Ca3A OH1A 2.304(3) 1_455 ?
Ca3A OH1 2.323(3) . ?
Ca3A O6A 2.383(3) . ?
Ca3A O5A 2.389(3) 3_656 ?
Ca3A O8 2.501(3) 4_556 ?
Ca3A O7 2.648(3) 4_556 ?
Ca3A O7A 2.726(3) 4_456 ?
Ca3A Si2 3.2599(16) 4_556 ?
Ca3A Si2A 3.2899(16) 4_456 ?
Ca3A O3A 3.457(3) 3_656 ?
Ca3A Si2A 3.511(2) 1_455 ?
Ca3A O9A 3.588(3) 1_455 ?
Ca3A H1 2.6634 . ?
Si1 O1A 1.601(3) 3_655 ?
Si1 O2 1.607(3) . ?
Si1 O9 1.608(3) . ?
Si1 O8A 1.643(3) . ?
Si1 Ca1 3.3157(18) 3_655 ?
Si1 Ca1A 3.6155(18) 3_655 ?
Si1A O1 1.592(3) 3_655 ?
Si1A O9A 1.608(3) . ?
Si1A O2A 1.610(3) 1_655 ?
Si1A O8A 1.647(3) . ?
Si1A Ca1 3.3083(18) 3_655 ?
Si1A Ca4 3.6003(17) 1_655 ?
Si1A Ca1A 3.6160(18) 3_755 ?
Si2 O6 1.576(3) . ?
Si2 O7 1.586(3) . ?
Si2 O9 1.641(3) . ?
Si2 O8 1.678(3) . ?
Si2 Ca3A 3.2599(16) 4 ?
Si2 Ca2 3.541(2) 4 ?
Si2 Ca3 3.6261(17) 4 ?
Si2A O7A 1.578(3) . ?
Si2A O6A 1.586(3) 1_655 ?
Si2A O9A 1.639(3) . ?
Si2A O8 1.666(3) 1_655 ?
Si2A Ca2 3.2762(16) 1_655 ?
Si2A Ca3A 3.2899(16) 4_655 ?
Si2A Ca3A 3.511(2) 1_655 ?
Si2A Ca2A 3.5618(19) 4 ?
C1 O5 1.256(6) . ?
C1 O4 1.291(5) . ?
C1 O3 1.307(5) . ?
C1A O5A 1.252(6) . ?
C1A O4A 1.295(5) . ?
C1A O3A 1.307(5) . ?
O1 Si1A 1.592(3) 3_655 ?
O1 Ca1A 2.328(4) 1_455 ?
O1 Ca1A 2.556(3) 3_655 ?
O1 O2A 2.605(5) 3 ?
O1 O8A 2.624(5) 3_655 ?
O1 O9A 2.692(4) 3_655 ?
O1 O1A 2.998(5) 3_655 ?
O1 O1 2.999(6) 3 ?
O1 O4 3.042(5) . ?
O1 OH2A 3.201(4) 1_455 ?
O1 OH2 3.246(4) . ?
O1A Si1 1.601(3) 3_655 ?
O1A Ca1 2.531(3) 3_655 ?
O1A O2 2.608(5) 3_655 ?
O1A O8A 2.641(4) 3_655 ?
O1A O9 2.686(4) 3_655 ?
O1A O1 2.998(5) 3_655 ?
O1A O1A 3.003(6) 3_655 ?
O1A O4A 3.024(5) . ?
O1A OH2A 3.200(4) . ?
O1A OH2 3.237(4) . ?
O2 O1A 2.608(5) 3_655 ?
O2 O8A 2.614(5) . ?
O2 O9 2.700(4) . ?
O2 O4 3.037(5) . ?
O2 O4A 3.041(5) . ?
O2 O3 3.051(4) 3_656 ?
O2 OH1 3.259(4) . ?
O2A Si1A 1.610(3) 1_455 ?
O2A Ca4A 2.398(4) 1_455 ?
O2A Ca1A 2.496(3) 1_455 ?
O2A O1 2.605(5) 3 ?
O2A O8A 2.632(4) 1_455 ?
O2A O9A 2.685(4) 1_455 ?
O2A O4 3.022(5) . ?
O2A O4A 3.035(5) 1_455 ?
O2A O3A 3.044(4) 3_656 ?
O2A OH1 3.245(4) . ?
O2A OH1A 3.295(4) 1_455 ?
O3 O4 2.219(5) . ?
O3 O5 2.232(4) . ?
O3 Ca4 2.492(4) 3_656 ?
O3 Ca4A 2.505(4) 3_656 ?
O3 O2 3.051(4) 3_656 ?
O3 O3A 3.074(6) 3_656 ?
O3 O3 3.081(7) 3_656 ?
O3 OH1A 3.293(4) 3_656 ?
O3 Ca3 3.432(3) 3_656 ?
O3A O4A 2.223(5) . ?
O3A O5A 2.230(4) . ?
O3A Ca4 2.493(4) 3_656 ?
O3A Ca4A 2.503(4) 3_756 ?
O3A O3A 3.039(7) 3_756 ?
O3A O2A 3.044(4) 3_656 ?
O3A O3 3.074(6) 3_656 ?
O3A OH1A 3.288(4) 3_756 ?
O3A Ca3A 3.457(3) 3_656 ?
O4 O5 2.222(4) . ?
O4 Ca1A 2.501(4) 1_455 ?
O4 OH2 3.232(4) . ?
O4 OH2A 3.270(5) 1_455 ?
O4 Ca2A 3.324(3) 2_655 ?
O4A O5A 2.221(4) . ?
O4A O2A 3.035(5) 1_655 ?
O4A OH2 3.223(5) . ?
O4A OH2A 3.283(4) . ?
O4A Ca2 3.351(3) 2_655 ?
O5 Ca3 2.393(3) 3_656 ?
O5 Ca2A 2.415(3) 2_655 ?
O5 OH1A 3.279(4) 3_656 ?
O5A Ca3A 2.389(3) 3_656 ?
O5A Ca2 2.397(3) 2_655 ?
O5A O8 2.930(5) 2_655 ?
O5A OH1A 3.252(4) 3_756 ?
O5A OH1 3.299(4) 3_656 ?
O5A OH2 3.300(4) . ?
O6 O8 2.540(4) . ?
O6 O9 2.666(4) . ?
O6 O7 2.754(4) . ?
O6 OH2 3.035(4) 2_645 ?
O6 O7A 3.130(4) 4_556 ?
O6 OH1A 3.178(4) . ?
O6A Si2A 1.586(3) 1_455 ?
O6A Ca2A 2.365(3) 1_455 ?
O6A O8 2.523(4) . ?
O6A O9A 2.666(4) 1_455 ?
O6A O7A 2.755(4) 1_455 ?
O6A OH2A 2.970(4) 2_645 ?
O6A OH1A 3.166(4) 1_455 ?
O7 Ca3 2.368(3) 4 ?
O7 Ca2 2.390(3) 4 ?
O7 O8 2.533(4) . ?
O7 Ca3A 2.648(3) 4 ?
O7 O9 2.675(4) . ?
O7 OH1 2.982(4) 4 ?
O7 OH2 3.155(4) 3_655 ?
O7A Ca3 2.338(3) 4 ?
O7A Ca2A 2.431(3) 4 ?
O7A O8 2.534(4) 1_655 ?
O7A O9A 2.671(4) . ?
O7A Ca3A 2.726(3) 4_655 ?
O7A O6A 2.755(4) 1_655 ?
O7A OH1A 3.028(4) 4 ?
O7A O6 3.130(4) 4 ?
O7A OH2 3.177(4) 3_655 ?
O8 Si2A 1.666(3) 1_455 ?
O8 Ca3A 2.501(3) 4 ?
O8 O7A 2.534(4) 1_455 ?
O8 O9A 2.630(4) 1_455 ?
O8 O9 2.636(4) . ?
O8 O5A 2.930(5) 2_645 ?
O8A O9 2.556(4) . ?
O8A O9A 2.561(4) . ?
O8A O1 2.624(5) 3_655 ?
O8A O2A 2.632(4) 1_655 ?
O8A O1A 2.641(4) 3_655 ?
O8A OH1A 2.911(3) . ?
O8A OH2 2.967(3) 3_655 ?
O8A Ca1 3.061(3) 3_655 ?
O9 O1A 2.686(4) 3_655 ?
O9 O9A 2.950(5) 1_455 ?
O9 OH2A 3.069(4) 3_655 ?
O9 OH1 3.108(4) . ?
O9A O8 2.630(4) 1_655 ?
O9A O6A 2.667(4) 1_655 ?
O9A O2A 2.685(4) 1_655 ?
O9A O1 2.692(4) 3_655 ?
O9A O9 2.950(5) 1_655 ?
O9A OH1 3.021(4) 1_655 ?
O9A OH2A 3.163(4) 3_755 ?
O9A Ca3A 3.588(3) 1_655 ?
OH1 O7 2.982(4) 4_556 ?
OH1 O9A 3.021(4) 1_455 ?
OH1 O5A 3.299(4) 3_656 ?
OH1 H1 0.8181 . ?
OH1A Ca3A 2.304(3) 1_655 ?
OH1A O7A 3.028(4) 4_556 ?
OH1A O6A 3.166(4) 1_655 ?
OH1A O5A 3.252(4) 3_756 ?
OH1A O5 3.279(4) 3_656 ?
OH1A O3A 3.288(4) 3_756 ?
OH1A O3 3.293(4) 3_656 ?
OH1A O2A 3.295(4) 1_655 ?
OH1A H1A 0.9012 . ?
OH2 Ca2 2.299(3) 2_655 ?
OH2 Ca2A 2.326(3) 2_655 ?
OH2 O8A 2.967(3) 3_655 ?
OH2 O6 3.035(4) 2_655 ?
OH2 O7 3.155(4) 3_655 ?
OH2 O7A 3.177(4) 3_655 ?
OH2 H2 0.8777 . ?
OH2A Ca2 2.312(3) 2_655 ?
OH2A Ca2A 2.340(3) 2_755 ?
OH2A O6A 2.970(4) 2_655 ?
OH2A O9 3.069(4) 3_655 ?
OH2A O9A 3.163(4) 3_755 ?
OH2A O1 3.201(4) 1_655 ?
OH2A O4 3.270(5) 1_655 ?
OH2A H2A 0.8705 . ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
OH2 Ca1 O1 87.92(10) . . ?
OH2 Ca1 O1A 86.82(10) . . ?
O1 Ca1 O1A 107.26(11) . . ?
OH2 Ca1 O4 84.56(10) . . ?
O1 Ca1 O4 77.48(12) . . ?
O1A Ca1 O4 170.02(10) . . ?
OH2 Ca1 O2 147.51(10) . . ?
O1 Ca1 O2 111.30(12) . . ?
O1A Ca1 O2 110.42(12) . . ?
O4 Ca1 O2 74.99(11) . . ?
OH2 Ca1 O4A 83.74(10) . . ?
O1 Ca1 O4A 170.93(11) . . ?
O1A Ca1 O4A 75.90(11) . . ?
O4 Ca1 O4A 98.12(11) . . ?
O2 Ca1 O4A 74.67(11) . . ?
OH2 Ca1 O1A 149.98(10) . 3_655 ?
O1 Ca1 O1A 75.39(11) . 3_655 ?
O1A Ca1 O1A 74.96(12) . 3_655 ?
O4 Ca1 O1A 114.96(12) . 3_655 ?
O2 Ca1 O1A 62.47(10) . 3_655 ?
O4A Ca1 O1A 113.68(12) . 3_655 ?
OH2 Ca1 Si1 172.77(10) . . ?
O1 Ca1 Si1 98.51(7) . . ?
O1A Ca1 Si1 88.10(7) . . ?
O4 Ca1 Si1 100.01(7) . . ?
O2 Ca1 Si1 31.81(7) . . ?
O4A Ca1 Si1 90.04(7) . . ?
O1A Ca1 Si1 31.69(7) 3_655 . ?
OH2 Ca1 O8A 65.34(8) . 3_655 ?
O1 Ca1 O8A 56.08(10) . 3_655 ?
O1A Ca1 O8A 56.30(10) . 3_655 ?
O4 Ca1 O8A 123.56(10) . 3_655 ?
O2 Ca1 O8A 147.14(9) . 3_655 ?
O4A Ca1 O8A 122.58(10) . 3_655 ?
O1A Ca1 O8A 84.66(9) 3_655 3_655 ?
Si1 Ca1 O8A 115.65(7) . 3_655 ?
OH2 Ca1 Si1A 74.29(7) . 3_655 ?
O1 Ca1 Si1A 26.51(8) . 3_655 ?
O1A Ca1 Si1A 83.69(9) . 3_655 ?
O4 Ca1 Si1A 98.76(9) . 3_655 ?
O2 Ca1 Si1A 133.02(9) . 3_655 ?
O4A Ca1 Si1A 150.74(8) . 3_655 ?
O1A Ca1 Si1A 80.07(8) 3_655 3_655 ?
Si1 Ca1 Si1A 110.25(4) . 3_655 ?
O8A Ca1 Si1A 29.66(6) 3_655 3_655 ?
OH2 Ca1 Si1 73.14(8) . 3_655 ?
O1 Ca1 Si1 83.47(9) . 3_655 ?
O1A Ca1 Si1 26.92(8) . 3_655 ?
O4 Ca1 Si1 151.11(8) . 3_655 ?
O2 Ca1 Si1 132.86(9) . 3_655 ?
O4A Ca1 Si1 97.45(9) . 3_655 ?
O1A Ca1 Si1 80.21(8) 3_655 3_655 ?
Si1 Ca1 Si1 104.16(4) . 3_655 ?
O8A Ca1 Si1 29.51(6) 3_655 3_655 ?
Si1A Ca1 Si1 58.06(4) 3_655 3_655 ?
OH2 Ca1 Ca1A 91.27(9) . 1_455 ?
O1 Ca1 Ca1A 36.75(8) . 1_455 ?
O1A Ca1 Ca1A 144.00(8) . 1_455 ?
O4 Ca1 Ca1A 41.51(8) . 1_455 ?
O2 Ca1 Ca1A 89.84(10) . 1_455 ?
O4A Ca1 Ca1A 139.62(9) . 1_455 ?
O1A Ca1 Ca1A 89.92(10) 3_655 1_455 ?
Si1 Ca1 Ca1A 95.87(4) . 1_455 ?
O8A Ca1 Ca1A 90.43(6) 3_655 1_455 ?
Si1A Ca1 Ca1A 61.33(4) 3_655 1_455 ?
Si1 Ca1 Ca1A 119.39(3) 3_655 1_455 ?
OH2 Ca1 H2 19.1 . . ?
O1 Ca1 H2 75.7 . . ?
O1A Ca1 H2 77.0 . . ?
O4 Ca1 H2 96.1 . . ?
O2 Ca1 H2 166.5 . . ?
O4A Ca1 H2 97.1 . . ?
O1A Ca1 H2 131.0 3_655 . ?
Si1 Ca1 H2 161.3 . . ?
O8A Ca1 H2 46.3 3_655 . ?
Si1A Ca1 H2 57.4 3_655 . ?
Si1 Ca1 H2 57.9 3_655 . ?
Ca1A Ca1 H2 89.9 1_455 . ?
O1 Ca1A OH2A 86.82(10) 1_655 . ?
O1 Ca1A O1A 106.17(11) 1_655 . ?
OH2A Ca1A O1A 86.42(10) . . ?
O1 Ca1A O2A 111.64(12) 1_655 1_655 ?
OH2A Ca1A O2A 148.25(10) . 1_655 ?
O1A Ca1A O2A 111.13(12) . 1_655 ?
O1 Ca1A O4 78.03(12) 1_655 1_655 ?
OH2A Ca1A O4 85.13(10) . 1_655 ?
O1A Ca1A O4 170.35(11) . 1_655 ?
O2A Ca1A O4 74.43(11) 1_655 1_655 ?
O1 Ca1A O4A 171.10(10) 1_655 . ?
OH2A Ca1A O4A 84.94(10) . . ?
O1A Ca1A O4A 76.68(11) . . ?
O2A Ca1A O4A 74.36(11) 1_655 . ?
O4 Ca1A O4A 97.90(11) 1_655 . ?
O1 Ca1A O1 75.63(12) 1_655 3_655 ?
OH2A Ca1A O1 149.68(10) . 3_655 ?
O1A Ca1A O1 75.32(12) . 3_655 ?
O2A Ca1A O1 62.07(10) 1_655 3_655 ?
O4 Ca1A O1 114.30(12) 1_655 3_655 ?
O4A Ca1A O1 113.26(12) . 3_655 ?
O1 Ca1A Si1A 98.79(7) 1_655 . ?
OH2A Ca1A Si1A 173.36(10) . . ?
O1A Ca1A Si1A 88.59(7) . . ?
O2A Ca1A Si1A 31.74(7) 1_655 . ?
O4 Ca1A Si1A 99.46(7) 1_655 . ?
O4A Ca1A Si1A 89.65(7) . . ?
O1 Ca1A Si1A 31.39(7) 3_655 . ?
O1 Ca1A Si1 90.81(9) 1_655 3_655 ?
OH2A Ca1A Si1 73.68(8) . 3_655 ?
O1A Ca1A Si1 19.22(8) . 3_655 ?
O2A Ca1A Si1 128.94(9) 1_655 3_655 ?
O4 Ca1A Si1 156.63(8) 1_655 3_655 ?
O4A Ca1A Si1 90.09(9) . 3_655 ?
O1 Ca1A Si1 81.92(8) 3_655 3_655 ?
Si1A Ca1A Si1 102.53(4) . 3_655 ?
O1 Ca1A Si1A 18.53(8) 1_655 3_755 ?
OH2A Ca1A Si1A 74.67(8) . 3_755 ?
O1A Ca1A Si1A 91.20(9) . 3_755 ?
O2A Ca1A Si1A 128.65(9) 1_655 3_755 ?
O4 Ca1A Si1A 91.06(9) 1_655 3_755 ?
O4A Ca1A Si1A 156.95(8) . 3_755 ?
O1 Ca1A Si1A 81.62(8) 3_655 3_755 ?
Si1A Ca1A Si1A 109.84(4) . 3_755 ?
Si1 Ca1A Si1A 74.13(4) 3_655 3_755 ?
O1 Ca1A Ca1 37.48(8) 1_655 1_655 ?
OH2A Ca1A Ca1 90.91(9) . 1_655 ?
O1A Ca1A Ca1 143.64(9) . 1_655 ?
O2A Ca1A Ca1 89.47(10) 1_655 1_655 ?
O4 Ca1A Ca1 41.33(9) 1_655 1_655 ?
O4A Ca1A Ca1 139.22(9) . 1_655 ?
O1 Ca1A Ca1 89.87(10) 3_655 1_655 ?
Si1A Ca1A Ca1 95.70(4) . 1_655 ?
Si1 Ca1A Ca1 127.52(4) 3_655 1_655 ?
Si1A Ca1A Ca1 53.39(3) 3_755 1_655 ?
O1 Ca1A Ca1 142.84(9) 1_655 . ?
OH2A Ca1A Ca1 89.16(9) . . ?
O1A Ca1A Ca1 36.68(8) . . ?
O2A Ca1A Ca1 90.30(10) 1_655 . ?
O4 Ca1A Ca1 138.36(9) 1_655 . ?
O4A Ca1A Ca1 40.47(8) . . ?
O1 Ca1A Ca1 90.24(10) 3_655 . ?
Si1A Ca1A Ca1 84.23(3) . . ?
Si1 Ca1A Ca1 52.80(4) 3_655 . ?
Si1A Ca1A Ca1 126.93(3) 3_755 . ?
Ca1 Ca1A Ca1 179.67(3) 1_655 . ?
O1 Ca1A H2A 74.8 1_655 . ?
OH2A Ca1A H2A 19.6 . . ?
O1A Ca1A H2A 75.6 . . ?
O2A Ca1A H2A 167.8 1_655 . ?
O4 Ca1A H2A 97.6 1_655 . ?
O4A Ca1A H2A 98.1 . . ?
O1 Ca1A H2A 130.1 3_655 . ?
Si1A Ca1A H2A 160.1 . . ?
Si1 Ca1A H2A 59.4 3_655 . ?
Si1A Ca1A H2A 59.5 3_755 . ?
Ca1 Ca1A H2A 90.3 1_655 . ?
Ca1 Ca1A H2A 89.9 . . ?
OH1 Ca4 O2A 88.50(10) . . ?
OH1 Ca4 O2 88.73(10) . . ?
O2A Ca4 O2 105.17(11) . . ?
OH1 Ca4 O3A 87.28(9) . 3_656 ?
O2A Ca4 O3A 78.13(11) . 3_656 ?
O2 Ca4 O3A 174.75(10) . 3_656 ?
OH1 Ca4 O3 86.88(10) . 3_656 ?
O2A Ca4 O3 174.24(10) . 3_656 ?
O2 Ca4 O3 78.17(11) . 3_656 ?
O3A Ca4 O3 98.20(11) 3_656 3_656 ?
OH1 Ca4 O3 153.29(9) . . ?
O2A Ca4 O3 107.31(12) . . ?
O2 Ca4 O3 106.94(12) . . ?
O3A Ca4 O3 75.54(12) 3_656 . ?
O3 Ca4 O3 75.76(12) 3_656 . ?
OH1 Ca4 O4 154.92(9) . . ?
O2A Ca4 O4 76.24(11) . . ?
O2 Ca4 O4 76.53(11) . . ?
O3A Ca4 O4 108.40(11) 3_656 . ?
O3 Ca4 O4 109.27(12) 3_656 . ?
O3 Ca4 O4 51.79(11) . . ?
OH1 Ca4 C1 179.14(10) . . ?
O2A Ca4 C1 91.49(10) . . ?
O2 Ca4 C1 92.10(10) . . ?
O3A Ca4 C1 91.88(10) 3_656 . ?
O3 Ca4 C1 93.08(10) 3_656 . ?
O3 Ca4 C1 26.04(9) . . ?
O4 Ca4 C1 25.75(9) . . ?
OH1 Ca4 Si1A 74.28(7) . 1_455 ?
O2A Ca4 Si1A 19.71(8) . 1_455 ?
O2 Ca4 Si1A 90.97(9) . 1_455 ?
O3A Ca4 Si1A 91.22(9) 3_656 1_455 ?
O3 Ca4 Si1A 158.53(8) 3_656 1_455 ?
O3 Ca4 Si1A 125.48(9) . 1_455 ?
O4 Ca4 Si1A 85.64(8) . 1_455 ?
C1 Ca4 Si1A 105.91(8) . 1_455 ?
OH1 Ca4 Si1 74.96(7) . . ?
O2A Ca4 Si1 90.97(9) . . ?
O2 Ca4 Si1 19.37(7) . . ?
O3A Ca4 Si1 159.47(8) 3_656 . ?
O3 Ca4 Si1 91.15(9) 3_656 . ?
O3 Ca4 Si1 124.68(9) . . ?
O4 Ca4 Si1 85.37(8) . . ?
C1 Ca4 Si1 105.89(8) . . ?
Si1A Ca4 Si1 74.30(4) 1_455 . ?
OH1 Ca4 Ca4A 90.19(8) . . ?
O2A Ca4 Ca4A 142.66(9) . . ?
O2 Ca4 Ca4A 37.49(8) . . ?
O3A Ca4 Ca4A 139.08(8) 3_656 . ?
O3 Ca4 Ca4A 40.88(8) 3_656 . ?
O3 Ca4 Ca4A 89.71(10) . . ?
O4 Ca4 Ca4A 90.17(10) . . ?
C1 Ca4 Ca4A 90.34(9) . . ?
Si1A Ca4 Ca4A 127.18(4) 1_455 . ?
Si1 Ca4 Ca4A 52.89(3) . . ?
OH1 Ca4 Ca4A 89.41(8) . 1_455 ?
O2A Ca4 Ca4A 37.42(8) . 1_455 ?
O2 Ca4 Ca4A 142.59(8) . 1_455 ?
O3A Ca4 Ca4A 40.80(8) 3_656 1_455 ?
O3 Ca4 Ca4A 138.99(9) 3_656 1_455 ?
O3 Ca4 Ca4A 90.61(10) . 1_455 ?
O4 Ca4 Ca4A 90.24(10) . 1_455 ?
C1 Ca4 Ca4A 90.06(9) . 1_455 ?
Si1A Ca4 Ca4A 52.77(3) 1_455 1_455 ?
Si1 Ca4 Ca4A 127.07(3) . 1_455 ?
Ca4A Ca4 Ca4A 179.58(3) . 1_455 ?
OH1 Ca4 H1 18.2 . . ?
O2A Ca4 H1 78.2 . . ?
O2 Ca4 H1 77.3 . . ?
O3A Ca4 H1 99.7 3_656 . ?
O3 Ca4 H1 98.2 3_656 . ?
O3 Ca4 H1 171.4 . . ?
O4 Ca4 H1 136.8 . . ?
C1 Ca4 H1 162.5 . . ?
Si1A Ca4 H1 61.1 1_455 . ?
Si1 Ca4 H1 60.7 . . ?
Ca4A Ca4 H1 89.5 . . ?
Ca4A Ca4 H1 90.2 1_455 . ?
OH1A Ca4A O2 90.11(10) . . ?
OH1A Ca4A O2A 89.31(10) . 1_655 ?
O2 Ca4A O2A 107.18(11) . 1_655 ?
OH1A Ca4A O3A 151.82(9) . . ?
O2 Ca4A O3A 106.80(12) . . ?
O2A Ca4A O3A 106.28(12) 1_655 . ?
OH1A Ca4A O3A 86.52(10) . 3_756 ?
O2 Ca4A O3A 174.82(10) . 3_756 ?
O2A Ca4A O3A 76.75(11) 1_655 3_756 ?
O3A Ca4A O3A 74.84(12) . 3_756 ?
OH1A Ca4A O3 86.66(10) . 3_656 ?
O2 Ca4A O3 76.94(11) . 3_656 ?
O2A Ca4A O3 174.26(10) 1_655 3_656 ?
O3A Ca4A O3 75.83(12) . 3_656 ?
O3A Ca4A O3 98.91(11) 3_756 3_656 ?
OH1A Ca4A O4A 155.66(9) . . ?
O2 Ca4A O4A 76.21(11) . . ?
O2A Ca4A O4A 76.02(11) 1_655 . ?
O3A Ca4A O4A 52.50(11) . . ?
O3A Ca4A O4A 108.30(11) 3_756 . ?
O3 Ca4A O4A 109.13(12) 3_656 . ?
OH1A Ca4A C1A 177.88(10) . . ?
O2 Ca4A C1A 91.86(10) . . ?
O2A Ca4A C1A 90.86(10) 1_655 . ?
O3A Ca4A C1A 26.37(9) . . ?
O3A Ca4A C1A 91.46(10) 3_756 . ?
O3 Ca4A C1A 93.02(10) 3_656 . ?
O4A Ca4A C1A 26.14(9) . . ?
OH1A Ca4A O8A 65.55(8) . . ?
O2 Ca4A O8A 56.93(10) . . ?
O2A Ca4A O8A 57.37(10) 1_655 . ?
O3A Ca4A O8A 142.63(9) . . ?
O3A Ca4A O8A 124.68(10) 3_756 . ?
O3 Ca4A O8A 124.08(10) 3_656 . ?
O4A Ca4A O8A 90.13(9) . . ?
C1A Ca4A O8A 116.26(9) . . ?
OH1A Ca4A Si1A 73.96(7) . . ?
O2 Ca4A Si1A 84.13(9) . . ?
O2A Ca4A Si1A 27.65(8) 1_655 . ?
O3A Ca4A Si1A 128.98(9) . . ?
O3A Ca4A Si1A 98.70(9) 3_756 . ?
O3 Ca4A Si1A 152.85(8) 3_656 . ?
O4A Ca4A Si1A 84.55(8) . . ?
C1A Ca4A Si1A 107.02(8) . . ?
O8A Ca4A Si1A 29.97(6) . . ?
OH1A Ca4A Si1 74.90(7) . . ?
O2 Ca4A Si1 27.34(8) . . ?
O2A Ca4A Si1 84.20(9) 1_655 . ?
O3A Ca4A Si1 128.93(9) . . ?
O3A Ca4A Si1 153.52(8) 3_756 . ?
O3 Ca4A Si1 98.66(9) 3_656 . ?
O4A Ca4A Si1 84.25(8) . . ?
C1A Ca4A Si1 107.22(8) . . ?
O8A Ca4A Si1 29.77(6) . . ?
Si1A Ca4A Si1 58.41(4) . . ?
OH1A Ca4A Ca4 90.94(8) . . ?
O2 Ca4A Ca4 36.51(8) . . ?
O2A Ca4A Ca4 143.68(8) 1_655 . ?
O3A Ca4A Ca4 89.88(10) . . ?
O3A Ca4A Ca4 139.51(9) 3_756 . ?
O3 Ca4A Ca4 40.62(8) 3_656 . ?
O4A Ca4A Ca4 89.75(10) . . ?
C1A Ca4A Ca4 90.18(9) . . ?
O8A Ca4A Ca4 90.04(6) . . ?
Si1A Ca4A Ca4 119.35(3) . . ?
Si1 Ca4A Ca4 60.94(4) . . ?
OH1A Ca4A H1A 20.0 . . ?
O2 Ca4A H1A 77.9 . . ?
O2A Ca4A H1A 78.1 1_655 . ?
O3A Ca4A H1A 171.8 . . ?
O3A Ca4A H1A 99.9 3_756 . ?
O3 Ca4A H1A 99.1 3_656 . ?
O4A Ca4A H1A 135.6 . . ?
C1A Ca4A H1A 161.8 . . ?
O8A Ca4A H1A 45.5 . . ?
Si1A Ca4A H1A 57.4 . . ?
Si1 Ca4A H1A 57.7 . . ?
Ca4 Ca4A H1A 90.3 . . ?
OH2 Ca2 OH2A 108.50(12) 2_645 2_645 ?
OH2 Ca2 O7 84.57(10) 2_645 4_556 ?
OH2A Ca2 O7 90.37(10) 2_645 4_556 ?
OH2 Ca2 O5A 89.26(10) 2_645 2_645 ?
OH2A Ca2 O5A 90.88(11) 2_645 2_645 ?
O7 Ca2 O5A 173.78(11) 4_556 2_645 ?
OH2 Ca2 O8 123.79(10) 2_645 . ?
OH2A Ca2 O8 124.26(10) 2_645 . ?
O7 Ca2 O8 111.02(9) 4_556 . ?
O5A Ca2 O8 73.14(10) 2_645 . ?
OH2 Ca2 O6A 171.58(10) 2_645 . ?
OH2A Ca2 O6A 73.00(10) 2_645 . ?
O7 Ca2 O6A 87.15(10) 4_556 . ?
O5A Ca2 O6A 99.05(10) 2_645 . ?
O8 Ca2 O6A 58.26(9) . . ?
OH2 Ca2 O6 73.35(10) 2_645 . ?
OH2A Ca2 O6 171.56(10) 2_645 . ?
O7 Ca2 O6 81.55(10) 4_556 . ?
O5A Ca2 O6 97.41(10) 2_645 . ?
O8 Ca2 O6 57.48(9) . . ?
O6A Ca2 O6 103.96(9) . . ?
OH2 Ca2 Si2A 153.66(8) 2_645 1_455 ?
OH2A Ca2 Si2A 96.79(9) 2_645 1_455 ?
O7 Ca2 Si2A 102.94(8) 4_556 1_455 ?
O5A Ca2 Si2A 82.96(8) 2_645 1_455 ?
O8 Ca2 Si2A 29.94(7) . 1_455 ?
O6A Ca2 Si2A 28.67(6) . 1_455 ?
O6 Ca2 Si2A 82.72(7) . 1_455 ?
OH2 Ca2 Si2 96.75(9) 2_645 . ?
OH2A Ca2 Si2 153.76(8) 2_645 . ?
O7 Ca2 Si2 99.22(8) 4_556 . ?
O5A Ca2 Si2 82.22(8) 2_645 . ?
O8 Ca2 Si2 29.60(7) . . ?
O6A Ca2 Si2 83.08(7) . . ?
O6 Ca2 Si2 28.19(6) . . ?
Si2A Ca2 Si2 57.33(4) 1_455 . ?
OH2 Ca2 O4A 66.58(10) 2_645 2_645 ?
OH2A Ca2 O4A 68.03(10) 2_645 2_645 ?
O7 Ca2 O4A 134.15(9) 4_556 2_645 ?
O5A Ca2 O4A 41.44(9) 2_645 2_645 ?
O8 Ca2 O4A 114.58(8) . 2_645 ?
O6A Ca2 O4A 120.92(10) . 2_645 ?
O6 Ca2 O4A 119.59(9) . 2_645 ?
Si2A Ca2 O4A 118.89(7) 1_455 2_645 ?
Si2 Ca2 O4A 118.18(7) . 2_645 ?
OH2 Ca2 Si2 81.43(7) 2_645 4_556 ?
OH2A Ca2 Si2 71.41(7) 2_645 4_556 ?
O7 Ca2 Si2 21.61(7) 4_556 4_556 ?
O5A Ca2 Si2 155.91(8) 2_645 4_556 ?
O8 Ca2 Si2 130.24(7) . 4_556 ?
O6A Ca2 Si2 91.39(6) . 4_556 ?
O6 Ca2 Si2 101.06(6) . 4_556 ?
Si2A Ca2 Si2 114.51(4) 1_455 4_556 ?
Si2 Ca2 Si2 120.78(4) . 4_556 ?
O4A Ca2 Si2 114.88(6) 2_645 4_556 ?
OH2 Ca2 Ca3 79.20(9) 2_645 . ?
OH2A Ca2 Ca3 129.92(8) 2_645 . ?
O7 Ca2 Ca3 40.04(7) 4_556 . ?
O5A Ca2 Ca3 139.20(9) 2_645 . ?
O8 Ca2 Ca3 81.16(7) . . ?
O6A Ca2 Ca3 93.46(7) . . ?
O6 Ca2 Ca3 41.79(6) . . ?
Si2A Ca2 Ca3 90.36(4) 1_455 . ?
Si2 Ca2 Ca3 60.87(4) . . ?
O4A Ca2 Ca3 145.60(8) 2_645 . ?
Si2 Ca2 Ca3 60.72(3) 4_556 . ?
OH2 Ca2A OH2A 110.43(12) 2_645 2_745 ?
OH2 Ca2A O6 81.02(11) 2_645 . ?
OH2A Ca2A O6 166.49(11) 2_745 . ?
OH2 Ca2A O6A 168.59(11) 2_645 1_655 ?
OH2A Ca2A O6A 78.30(11) 2_745 1_655 ?
O6 Ca2A O6A 89.47(10) . 1_655 ?
OH2 Ca2A O5 89.05(10) 2_645 2_645 ?
OH2A Ca2A O5 90.85(10) 2_745 2_645 ?
O6 Ca2A O5 96.64(10) . 2_645 ?
O6A Ca2A O5 98.35(10) 1_655 2_645 ?
OH2 Ca2A O7A 83.77(10) 2_645 4_556 ?
OH2A Ca2A O7A 92.07(10) 2_745 4_556 ?
O6 Ca2A O7A 81.84(10) . 4_556 ?
O6A Ca2A O7A 88.68(10) 1_655 4_556 ?
O5 Ca2A O7A 172.80(11) 2_645 4_556 ?
OH2 Ca2A O4 67.11(10) 2_645 2_645 ?
OH2A Ca2A O4 67.99(10) 2_745 2_645 ?
O6 Ca2A O4 124.60(10) . 2_645 ?
O6A Ca2A O4 124.00(10) 1_655 2_645 ?
O5 Ca2A O4 41.93(9) 2_645 2_645 ?
O7A Ca2A O4 134.04(9) 4_556 2_645 ?
OH2 Ca2A Si2A 82.68(7) 2_645 4_556 ?
OH2A Ca2A Si2A 72.48(7) 2_745 4_556 ?
O6 Ca2A Si2A 102.91(7) . 4_556 ?
O6A Ca2A Si2A 93.41(7) 1_655 4_556 ?
O5 Ca2A Si2A 157.24(8) 2_645 4_556 ?
O7A Ca2A Si2A 21.57(7) 4_556 4_556 ?
O4 Ca2A Si2A 115.71(6) 2_645 4_556 ?
OH2 Ca2A Ca3 79.63(8) 2_645 . ?
OH2A Ca2A Ca3 131.12(8) 2_745 . ?
O6 Ca2A Ca3 41.77(7) . . ?
O6A Ca2A Ca3 89.08(8) 1_655 . ?
O5 Ca2A Ca3 137.91(8) 2_645 . ?
O7A Ca2A Ca3 40.07(7) 4_556 . ?
O4 Ca2A Ca3 146.52(8) 2_645 . ?
Si2A Ca2A Ca3 61.26(3) 4_556 . ?
OH2 Ca2A Ca3A 132.40(8) 2_645 1_655 ?
OH2A Ca2A Ca3A 78.19(8) 2_745 1_655 ?
O6 Ca2A Ca3A 88.80(8) . 1_655 ?
O6A Ca2A Ca3A 40.35(7) 1_655 1_655 ?
O5 Ca2A Ca3A 138.46(8) 2_645 1_655 ?
O7A Ca2A Ca3A 48.69(7) 4_556 1_655 ?
O4 Ca2A Ca3A 145.91(8) 2_645 1_655 ?
Si2A Ca2A Ca3A 54.45(3) 4_556 1_655 ?
Ca3 Ca2A Ca3A 63.01(3) . 1_655 ?
OH2 Ca2A O9A 71.37(8) 2_645 4_556 ?
OH2A Ca2A O9A 58.22(8) 2_745 4_556 ?
O6 Ca2A O9A 122.20(9) . 4_556 ?
O6A Ca2A O9A 109.17(9) 1_655 4_556 ?
O5 Ca2A O9A 131.31(10) 2_645 4_556 ?
O7A Ca2A O9A 46.28(8) 4_556 4_556 ?
O4 Ca2A O9A 89.67(7) 2_645 4_556 ?
Si2A Ca2A O9A 26.04(5) 4_556 4_556 ?
Ca3 Ca2A O9A 83.09(5) . 4_556 ?
Ca3A Ca2A O9A 75.61(5) 1_655 4_556 ?
OH2 Ca2A Ca2 34.97(8) 2_645 . ?
OH2A Ca2A Ca2 145.39(8) 2_745 . ?
O6 Ca2A Ca2 46.36(7) . . ?
O6A Ca2A Ca2 135.82(8) 1_655 . ?
O5 Ca2A Ca2 89.29(8) 2_645 . ?
O7A Ca2A Ca2 84.57(8) 4_556 . ?
O4 Ca2A Ca2 89.91(8) 2_645 . ?
Si2A Ca2A Ca2 95.77(4) 4_556 . ?
Ca3 Ca2A Ca2 58.91(3) . . ?
Ca3A Ca2A Ca2 121.93(4) 1_655 . ?
O9A Ca2A Ca2 97.12(5) 4_556 . ?
OH1A Ca3 O7A 80.84(11) . 4_556 ?
OH1A Ca3 OH1 109.91(11) . . ?
O7A Ca3 OH1 167.76(11) 4_556 . ?
OH1A Ca3 O7 169.47(11) . 4_556 ?
O7A Ca3 O7 90.24(10) 4_556 4_556 ?
OH1 Ca3 O7 78.45(11) . 4_556 ?
OH1A Ca3 O5 87.87(10) . 3_656 ?
O7A Ca3 O5 98.08(10) 4_556 3_656 ?
OH1 Ca3 O5 88.39(10) . 3_656 ?
O7 Ca3 O5 99.00(11) 4_556 3_656 ?
OH1A Ca3 O6 83.94(10) . . ?
O7A Ca3 O6 82.26(10) 4_556 . ?
OH1 Ca3 O6 92.85(10) . . ?
O7 Ca3 O6 89.35(10) 4_556 . ?
O5 Ca3 O6 171.64(11) 3_656 . ?
OH1A Ca3 O3 66.54(10) . 3_656 ?
O7A Ca3 O3 124.36(10) 4_556 3_656 ?
OH1 Ca3 O3 66.83(10) . 3_656 ?
O7 Ca3 O3 123.67(10) 4_556 3_656 ?
O5 Ca3 O3 40.31(9) 3_656 3_656 ?
O6 Ca3 O3 133.36(9) . 3_656 ?
OH1A Ca3 Si2 82.73(7) . . ?
O7A Ca3 Si2 103.80(7) 4_556 . ?
OH1 Ca3 Si2 72.75(6) . . ?
O7 Ca3 Si2 94.07(7) 4_556 . ?
O5 Ca3 Si2 154.41(8) 3_656 . ?
O6 Ca3 Si2 22.09(7) . . ?
O3 Ca3 Si2 114.56(6) 3_656 . ?
OH1A Ca3 Ca2A 80.23(8) . . ?
O7A Ca3 Ca2A 42.03(7) 4_556 . ?
OH1 Ca3 Ca2A 132.04(7) . . ?
O7 Ca3 Ca2A 89.40(8) 4_556 . ?
O5 Ca3 Ca2A 139.54(9) 3_656 . ?
O6 Ca3 Ca2A 40.24(7) . . ?
O3 Ca3 Ca2A 146.60(8) 3_656 . ?
Si2 Ca3 Ca2A 61.96(3) . . ?
OH1A Ca3 Si2 160.27(7) . 4_556 ?
O7A Ca3 Si2 83.59(8) 4_556 4_556 ?
OH1 Ca3 Si2 87.01(8) . 4_556 ?
O7 Ca3 Si2 18.96(7) 4_556 4_556 ?
O5 Ca3 Si2 82.37(8) 3_656 4_556 ?
O6 Ca3 Si2 105.94(8) . 4_556 ?
O3 Ca3 Si2 113.87(7) 3_656 4_556 ?
Si2 Ca3 Si2 112.88(4) . 4_556 ?
Ca2A Ca3 Si2 96.17(4) . 4_556 ?
OH1A Ca3 Ca2 133.04(7) . . ?
O7A Ca3 Ca2 89.35(8) 4_556 . ?
OH1 Ca3 Ca2 79.04(8) . . ?
O7 Ca3 Ca2 40.49(7) 4_556 . ?
O5 Ca3 Ca2 139.08(9) 3_656 . ?
O6 Ca3 Ca2 49.17(7) . . ?
O3 Ca3 Ca2 145.64(8) 3_656 . ?
Si2 Ca3 Ca2 55.16(3) . . ?
Ca2A Ca3 Ca2 63.04(3) . . ?
Si2 Ca3 Ca2 58.42(4) 4_556 . ?
OH1A Ca3 O9 71.33(8) . . ?
O7A Ca3 O9 123.25(9) 4_556 . ?
OH1 Ca3 O9 57.95(8) . . ?
O7 Ca3 O9 109.69(9) 4_556 . ?
O5 Ca3 O9 128.09(10) 3_656 . ?
O6 Ca3 O9 47.20(8) . . ?
O3 Ca3 O9 88.14(7) 3_656 . ?
Si2 Ca3 O9 26.43(5) . . ?
Ca2A Ca3 O9 84.28(6) . . ?
Si2 Ca3 O9 127.91(6) 4_556 . ?
Ca2 Ca3 O9 76.59(5) . . ?
OH1A Ca3 H1 103.5 . . ?
O7A Ca3 H1 156.7 4_556 . ?
OH1 Ca3 H1 17.8 . . ?
O7 Ca3 H1 82.6 4_556 . ?
O5 Ca3 H1 104.9 3_656 . ?
O6 Ca3 H1 75.5 . . ?
O3 Ca3 H1 77.3 3_656 . ?
Si2 Ca3 H1 55.0 . . ?
Ca2A Ca3 H1 115.4 . . ?
Si2 Ca3 H1 95.6 4_556 . ?
Ca2 Ca3 H1 70.8 . . ?
O9 Ca3 H1 41.6 . . ?
OH1A Ca3 H1A 19.7 . . ?
O7A Ca3 H1A 85.4 4_556 . ?
OH1 Ca3 H1A 102.8 . . ?
O7 Ca3 H1A 154.7 4_556 . ?
O5 Ca3 H1A 106.3 3_656 . ?
O6 Ca3 H1A 65.4 . . ?
O3 Ca3 H1A 78.3 3_656 . ?
Si2 Ca3 H1A 63.1 . . ?
Ca2A Ca3 H1A 70.8 . . ?
Si2 Ca3 H1A 166.9 4_556 . ?
Ca2 Ca3 H1A 114.4 . . ?
O9 Ca3 H1A 54.3 . . ?
H1 Ca3 H1A 91.6 . . ?
OH1A Ca3A OH1 107.98(11) 1_455 . ?
OH1A Ca3A O6A 84.94(10) 1_455 . ?
OH1 Ca3A O6A 91.35(10) . . ?
OH1A Ca3A O5A 87.69(10) 1_455 3_656 ?
OH1 Ca3A O5A 88.86(10) . 3_656 ?
O6A Ca3A O5A 172.33(11) . 3_656 ?
OH1A Ca3A O8 123.31(10) 1_455 4_556 ?
OH1 Ca3A O8 124.07(10) . 4_556 ?
O6A Ca3A O8 112.41(9) . 4_556 ?
O5A Ca3A O8 73.59(10) 3_656 4_556 ?
OH1A Ca3A O7 172.38(10) 1_455 4_556 ?
OH1 Ca3A O7 73.40(10) . 4_556 ?
O6A Ca3A O7 87.54(10) . 4_556 ?
O5A Ca3A O7 99.86(10) 3_656 4_556 ?
O8 Ca3A O7 58.84(9) 4_556 4_556 ?
OH1A Ca3A O7A 73.49(10) 1_455 4_456 ?
OH1 Ca3A O7A 172.80(9) . 4_456 ?
O6A Ca3A O7A 81.72(9) . 4_456 ?
O5A Ca3A O7A 98.26(10) 3_656 4_456 ?
O8 Ca3A O7A 57.81(9) 4_556 4_456 ?
O7 Ca3A O7A 104.19(9) 4_556 4_456 ?
OH1A Ca3A Si2 153.68(8) 1_455 4_556 ?
OH1 Ca3A Si2 96.64(8) . 4_556 ?
O6A Ca3A Si2 104.02(8) . 4_556 ?
O5A Ca3A Si2 83.57(8) 3_656 4_556 ?
O8 Ca3A Si2 30.40(7) 4_556 4_556 ?
O7 Ca3A Si2 28.83(6) 4_556 4_556 ?
O7A Ca3A Si2 83.24(7) 4_456 4_556 ?
OH1A Ca3A Si2A 96.59(8) 1_455 4_456 ?
OH1 Ca3A Si2A 153.70(8) . 4_456 ?
O6A Ca3A Si2A 100.20(8) . 4_456 ?
O5A Ca3A Si2A 82.77(8) 3_656 4_456 ?
O8 Ca3A Si2A 29.65(7) 4_556 4_456 ?
O7 Ca3A Si2A 83.49(7) 4_556 4_456 ?
O7A Ca3A Si2A 28.50(6) 4_456 4_456 ?
Si2 Ca3A Si2A 57.74(4) 4_556 4_456 ?
OH1A Ca3A O3A 66.10(10) 1_455 3_656 ?
OH1 Ca3A O3A 66.85(10) . 3_656 ?
O6A Ca3A O3A 133.91(8) . 3_656 ?
O5A Ca3A O3A 39.83(9) 3_656 3_656 ?
O8 Ca3A O3A 113.42(8) 4_556 3_656 ?
O7 Ca3A O3A 120.61(10) 4_556 3_656 ?
O7A Ca3A O3A 119.56(10) 4_456 3_656 ?
Si2 Ca3A O3A 117.96(7) 4_556 3_656 ?
Si2A Ca3A O3A 117.39(7) 4_456 3_656 ?
OH1A Ca3A Si2A 81.62(7) 1_455 1_455 ?
OH1 Ca3A Si2A 71.76(7) . 1_455 ?
O6A Ca3A Si2A 22.23(7) . 1_455 ?
O5A Ca3A Si2A 153.52(8) 3_656 1_455 ?
O8 Ca3A Si2A 132.20(7) 4_556 1_455 ?
O7 Ca3A Si2A 91.88(6) 4_556 1_455 ?
O7A Ca3A Si2A 101.76(6) 4_456 1_455 ?
Si2 Ca3A Si2A 115.75(4) 4_556 1_455 ?
Si2A Ca3A Si2A 122.37(4) 4_456 1_455 ?
O3A Ca3A Si2A 114.06(6) 3_656 1_455 ?
OH1A Ca3A O9A 69.89(8) 1_455 1_455 ?
OH1 Ca3A O9A 56.74(8) . 1_455 ?
O6A Ca3A O9A 47.99(8) . 1_455 ?
O5A Ca3A O9A 126.92(10) 3_656 1_455 ?
O8 Ca3A O9A 158.20(8) 4_556 1_455 ?
O7 Ca3A O9A 105.78(8) 4_556 1_455 ?
O7A Ca3A O9A 118.56(8) 4_456 1_455 ?
Si2 Ca3A O9A 134.09(6) 4_556 1_455 ?
Si2A Ca3A O9A 144.93(6) 4_456 1_455 ?
O3A Ca3A O9A 87.40(7) 3_656 1_455 ?
Si2A Ca3A O9A 26.67(5) 1_455 1_455 ?
OH1A Ca3A H1 102.2 1_455 . ?
OH1 Ca3A H1 17.2 . . ?
O6A Ca3A H1 74.6 . . ?
O5A Ca3A H1 105.0 3_656 . ?
O8 Ca3A H1 134.0 4_556 . ?
O7 Ca3A H1 76.9 4_556 . ?
O7A Ca3A H1 156.2 4_456 . ?
Si2 Ca3A H1 104.0 4_556 . ?
Si2A Ca3A H1 159.8 4_456 . ?
O3A Ca3A H1 77.5 3_656 . ?
Si2A Ca3A H1 54.6 1_455 . ?
O9A Ca3A H1 41.3 1_455 . ?
O1A Si1 O2 108.79(17) 3_655 . ?
O1A Si1 O9 113.63(17) 3_655 . ?
O2 Si1 O9 114.20(17) . . ?
O1A Si1 O8A 109.05(18) 3_655 . ?
O2 Si1 O8A 107.09(18) . . ?
O9 Si1 O8A 103.68(17) . . ?
O1A Si1 Ca1 56.18(10) 3_655 . ?
O2 Si1 Ca1 55.00(10) . . ?
O9 Si1 Ca1 148.07(13) . . ?
O8A Si1 Ca1 108.23(12) . . ?
O1A Si1 Ca4A 127.94(12) 3_655 . ?
O2 Si1 Ca4A 43.23(14) . . ?
O9 Si1 Ca4A 118.10(12) . . ?
O8A Si1 Ca4A 64.28(9) . . ?
Ca1 Si1 Ca4A 76.28(3) . . ?
O1A Si1 Ca1 42.76(15) 3_655 3_655 ?
O2 Si1 Ca1 126.42(12) . 3_655 ?
O9 Si1 Ca1 118.98(12) . 3_655 ?
O8A Si1 Ca1 66.62(9) . 3_655 ?
Ca1 Si1 Ca1 75.84(4) . 3_655 ?
Ca4A Si1 Ca1 110.47(5) . 3_655 ?
O1A Si1 Ca1A 28.81(14) 3_655 3_655 ?
O2 Si1 Ca1A 109.31(13) . 3_655 ?
O9 Si1 Ca1A 88.74(12) . 3_655 ?
O8A Si1 Ca1A 132.06(10) . 3_655 ?
Ca1 Si1 Ca1A 70.64(3) . 3_655 ?
Ca4A Si1 Ca1A 146.44(5) . 3_655 ?
Ca1 Si1 Ca1A 66.91(4) 3_655 3_655 ?
O1A Si1 Ca4 110.80(14) 3_655 . ?
O2 Si1 Ca4 28.92(14) . . ?
O9 Si1 Ca4 88.43(12) . . ?
O8A Si1 Ca4 128.81(9) . . ?
Ca1 Si1 Ca4 70.95(3) . . ?
Ca4A Si1 Ca4 66.18(4) . . ?
Ca1 Si1 Ca4 146.45(5) 3_655 . ?
Ca1A Si1 Ca4 97.09(5) 3_655 . ?
O1 Si1A O9A 114.56(17) 3_655 . ?
O1 Si1A O2A 108.92(17) 3_655 1_655 ?
O9A Si1A O2A 113.14(17) . 1_655 ?
O1 Si1A O8A 108.22(18) 3_655 . ?
O9A Si1A O8A 103.76(17) . . ?
O2A Si1A O8A 107.82(18) 1_655 . ?
O1 Si1A Ca1A 56.78(10) 3_655 . ?
O9A Si1A Ca1A 148.31(13) . . ?
O2A Si1A Ca1A 54.66(10) 1_655 . ?
O8A Si1A Ca1A 107.86(12) . . ?
O1 Si1A Ca4A 128.78(13) 3_655 . ?
O9A Si1A Ca4A 116.33(11) . . ?
O2A Si1A Ca4A 43.75(14) 1_655 . ?
O8A Si1A Ca4A 64.66(9) . . ?
Ca1A Si1A Ca4A 76.58(4) . . ?
O1 Si1A Ca1 41.61(15) 3_655 3_655 ?
O9A Si1A Ca1 120.65(12) . 3_655 ?
O2A Si1A Ca1 125.73(12) 1_655 3_655 ?
O8A Si1A Ca1 66.82(9) . 3_655 ?
Ca1A Si1A Ca1 75.02(4) . 3_655 ?
Ca4A Si1A Ca1 110.98(5) . 3_655 ?
O1 Si1A Ca4 111.22(14) 3_655 1_655 ?
O9A Si1A Ca4 87.07(12) . 1_655 ?
O2A Si1A Ca4 29.27(13) 1_655 1_655 ?
O8A Si1A Ca4 129.67(10) . 1_655 ?
Ca1A Si1A Ca4 71.28(3) . 1_655 ?
Ca4A Si1A Ca4 66.53(4) . 1_655 ?
Ca1 Si1A Ca4 145.81(5) 3_655 1_655 ?
O1 Si1A Ca1A 27.70(14) 3_655 3_755 ?
O9A Si1A Ca1A 90.77(11) . 3_755 ?
O2A Si1A Ca1A 108.92(14) 1_655 3_755 ?
O8A Si1A Ca1A 130.69(9) . 3_755 ?
Ca1A Si1A Ca1A 70.16(4) . 3_755 ?
Ca4A Si1A Ca1A 146.35(5) . 3_755 ?
Ca1 Si1A Ca1A 65.28(4) 3_655 3_755 ?
Ca4 Si1A Ca1A 97.40(5) 1_655 3_755 ?
O6 Si2 O7 121.11(17) . . ?
O6 Si2 O9 111.90(15) . . ?
O7 Si2 O9 112.02(15) . . ?
O6 Si2 O8 102.54(14) . . ?
O7 Si2 O8 101.73(15) . . ?
O9 Si2 O8 105.17(16) . . ?
O6 Si2 Ca3A 117.48(11) . 4 ?
O7 Si2 Ca3A 53.65(11) . 4 ?
O9 Si2 Ca3A 127.71(12) . 4 ?
O8 Si2 Ca3A 48.92(9) . 4 ?
O6 Si2 Ca2 55.42(11) . . ?
O7 Si2 Ca2 117.26(12) . . ?
O9 Si2 Ca2 127.14(12) . . ?
O8 Si2 Ca2 47.83(9) . . ?
Ca3A Si2 Ca2 73.34(4) 4 . ?
O6 Si2 Ca3 35.25(10) . . ?
O7 Si2 Ca3 153.61(12) . . ?
O9 Si2 Ca3 80.29(11) . . ?
O8 Si2 Ca3 96.98(9) . . ?
Ca3A Si2 Ca3 137.26(5) 4 . ?
Ca2 Si2 Ca3 63.97(4) . . ?
O6 Si2 Ca2 150.65(12) . 4 ?
O7 Si2 Ca2 33.72(10) . 4 ?
O9 Si2 Ca2 80.66(11) . 4 ?
O8 Si2 Ca2 99.19(8) . 4 ?
Ca3A Si2 Ca2 64.77(3) 4 4 ?
Ca2 Si2 Ca2 138.07(5) . 4 ?
Ca3 Si2 Ca2 157.65(5) . 4 ?
O6 Si2 Ca3 92.18(11) . 4 ?
O7 Si2 Ca3 29.03(11) . 4 ?
O9 Si2 Ca3 128.23(12) . 4 ?
O8 Si2 Ca3 113.55(10) . 4 ?
Ca3A Si2 Ca3 66.68(4) 4 4 ?
Ca2 Si2 Ca3 104.43(5) . 4 ?
Ca3 Si2 Ca3 125.19(5) . 4 ?
Ca2 Si2 Ca3 60.86(3) 4 4 ?
O7A Si2A O6A 121.06(17) . 1_655 ?
O7A Si2A O9A 112.23(15) . . ?
O6A Si2A O9A 111.50(15) 1_655 . ?
O7A Si2A O8 102.65(15) . 1_655 ?
O6A Si2A O8 101.71(15) 1_655 1_655 ?
O9A Si2A O8 105.39(16) . 1_655 ?
O7A Si2A Ca2 117.87(11) . 1_655 ?
O6A Si2A Ca2 53.53(11) 1_655 1_655 ?
O9A Si2A Ca2 127.19(12) . 1_655 ?
O8 Si2A Ca2 48.96(9) 1_655 1_655 ?
O7A Si2A Ca3A 55.48(11) . 4_655 ?
O6A Si2A Ca3A 117.02(12) 1_655 4_655 ?
O9A Si2A Ca3A 127.92(12) . 4_655 ?
O8 Si2A Ca3A 47.93(9) 1_655 4_655 ?
Ca2 Si2A Ca3A 73.48(4) 1_655 4_655 ?
O7A Si2A Ca3A 151.24(12) . 1_655 ?
O6A Si2A Ca3A 34.64(10) 1_655 1_655 ?
O9A Si2A Ca3A 79.29(11) . 1_655 ?
O8 Si2A Ca3A 99.09(8) 1_655 1_655 ?
Ca2 Si2A Ca3A 64.96(3) 1_655 1_655 ?
Ca3A Si2A Ca3A 138.38(5) 4_655 1_655 ?
O7A Si2A Ca2A 34.50(10) . 4 ?
O6A Si2A Ca2A 152.96(12) 1_655 4 ?
O9A Si2A Ca2A 81.43(11) . 4 ?
O8 Si2A Ca2A 97.15(9) 1_655 4 ?
Ca2 Si2A Ca2A 137.25(4) 1_655 4 ?
Ca3A Si2A Ca2A 63.81(4) 4_655 4 ?
Ca3A Si2A Ca2A 157.47(5) 1_655 4 ?
O5 C1 O4 121.5(3) . . ?
O5 C1 O3 121.1(3) . . ?
O4 C1 O3 117.3(4) . . ?
O5 C1 Ca4 178.5(3) . . ?
O4 C1 Ca4 59.3(2) . . ?
O3 C1 Ca4 58.1(2) . . ?
O5A C1A O4A 121.4(3) . . ?
O5A C1A O3A 121.2(3) . . ?
O4A C1A O3A 117.4(4) . . ?
O5A C1A Ca4A 178.8(3) . . ?
O4A C1A Ca4A 59.3(2) . . ?
O3A C1A Ca4A 58.1(2) . . ?
Si1A O1 Ca1A 133.8(2) 3_655 1_455 ?
Si1A O1 Ca1 111.9(2) 3_655 . ?
Ca1A O1 Ca1 105.77(12) 1_455 . ?
Si1A O1 Ca1A 91.83(13) 3_655 3_655 ?
Ca1A O1 Ca1A 104.37(12) 1_455 3_655 ?
Ca1 O1 Ca1A 103.91(12) . 3_655 ?
Si1A O1 O2A 35.77(10) 3_655 3 ?
Ca1A O1 O2A 126.7(2) 1_455 3 ?
Ca1 O1 O2A 126.7(2) . 3 ?
Ca1A O1 O2A 57.83(8) 3_655 3 ?
Si1A O1 O8A 36.61(11) 3_655 3_655 ?
Ca1A O1 O8A 157.11(14) 1_455 3_655 ?
Ca1 O1 O8A 75.45(13) . 3_655 ?
Ca1A O1 O8A 97.31(13) 3_655 3_655 ?
O2A O1 O8A 60.44(13) 3 3_655 ?
Si1A O1 O9A 32.91(10) 3_655 3_655 ?
Ca1A O1 O9A 104.58(14) 1_455 3_655 ?
Ca1 O1 O9A 118.62(14) . 3_655 ?
Ca1A O1 O9A 118.13(13) 3_655 3_655 ?
O2A O1 O9A 60.89(10) 3 3_655 ?
O8A O1 O9A 57.59(11) 3_655 3_655 ?
Si1A O1 O1A 108.0(2) 3_655 3_655 ?
Ca1A O1 O1A 115.42(13) 1_455 3_655 ?
Ca1 O1 O1A 54.79(11) . 3_655 ?
Ca1A O1 O1A 49.13(8) 3_655 3_655 ?
O2A O1 O1A 90.60(14) 3 3_655 ?
O8A O1 O1A 84.39(16) 3_655 3_655 ?
O9A O1 O1A 139.80(18) 3_655 3_655 ?
Si1A O1 O1 124.3(2) 3_655 3 ?
Ca1A O1 O1 55.64(12) 1_455 3 ?
Ca1 O1 O1 114.57(15) . 3 ?
Ca1A O1 O1 48.74(8) 3_655 3 ?
O2A O1 O1 90.55(15) 3 3 ?
O8A O1 O1 145.42(17) 3_655 3 ?
O9A O1 O1 126.7(2) 3_655 3 ?
O1A O1 O1 77.02(12) 3_655 3 ?
Si1A O1 O4 144.42(16) 3_655 . ?
Ca1A O1 O4 53.52(11) 1_455 . ?
Ca1 O1 O4 53.09(10) . . ?
Ca1A O1 O4 121.88(10) 3_655 . ?
O2A O1 O4 179.65(19) 3 . ?
O8A O1 O4 119.53(17) 3_655 . ?
O9A O1 O4 119.42(11) 3_655 . ?
O1A O1 O4 89.05(13) 3_655 . ?
O1 O1 O4 89.36(14) 3 . ?
Si1A O1 OH2A 97.17(14) 3_655 1_455 ?
Ca1A O1 OH2A 46.63(8) 1_455 1_455 ?
Ca1 O1 OH2A 104.81(11) . 1_455 ?
Ca1A O1 OH2A 143.99(16) 3_655 1_455 ?
O2A O1 OH2A 117.23(15) 3 1_455 ?
O8A O1 OH2A 110.57(12) 3_655 1_455 ?
O9A O1 OH2A 64.26(10) 3_655 1_455 ?
O1A O1 OH2A 152.06(14) 3_655 1_455 ?
O1 O1 OH2A 99.00(18) 3 1_455 ?
O4 O1 OH2A 63.12(10) . 1_455 ?
Si1A O1 OH2 84.84(14) 3_655 . ?
Ca1A O1 OH2 104.46(11) 1_455 . ?
Ca1 O1 OH2 45.29(8) . . ?
Ca1A O1 OH2 142.82(16) 3_655 . ?
O2A O1 OH2 118.31(15) 3 . ?
O8A O1 OH2 59.60(10) 3_655 . ?
O9A O1 OH2 76.02(11) 3_655 . ?
O1A O1 OH2 96.88(16) 3_655 . ?
O1 O1 OH2 150.78(16) 3 . ?
O4 O1 OH2 61.76(10) . . ?
OH2A O1 OH2 72.94(10) 1_455 . ?
Si1 O1A Ca1A 132.0(2) 3_655 . ?
Si1 O1A Ca1 110.3(2) 3_655 . ?
Ca1A O1A Ca1 107.64(12) . . ?
Si1 O1A Ca1 92.12(13) 3_655 3_655 ?
Ca1A O1A Ca1 105.37(13) . 3_655 ?
Ca1 O1A Ca1 105.04(12) . 3_655 ?
Si1 O1A O2 35.69(10) 3_655 3_655 ?
Ca1A O1A O2 126.1(2) . 3_655 ?
Ca1 O1A O2 125.9(2) . 3_655 ?
Ca1 O1A O2 58.14(8) 3_655 3_655 ?
Si1 O1A O8A 36.00(11) 3_655 3_655 ?
Ca1A O1A O8A 155.40(14) . 3_655 ?
Ca1 O1A O8A 74.59(12) . 3_655 ?
Ca1 O1A O8A 97.36(13) 3_655 3_655 ?
O2 O1A O8A 59.72(12) 3_655 3_655 ?
Si1 O1A O9 33.27(10) 3_655 3_655 ?
Ca1A O1A O9 102.37(14) . 3_655 ?
Ca1 O1A O9 116.60(14) . 3_655 ?
Ca1 O1A O9 118.79(13) 3_655 3_655 ?
O2 O1A O9 61.31(10) 3_655 3_655 ?
O8A O1A O9 57.34(11) 3_655 3_655 ?
Si1 O1A O1 124.64(19) 3_655 3_655 ?
Ca1A O1A O1 55.56(11) . 3_655 ?
Ca1 O1A O1 116.96(13) . 3_655 ?
Ca1 O1A O1 49.82(8) 3_655 3_655 ?
O2 O1A O1 91.28(14) 3_655 3_655 ?
O8A O1A O1 146.26(15) 3_655 3_655 ?
O9 O1A O1 126.12(19) 3_655 3_655 ?
Si1 O1A O1A 108.0(2) 3_655 3_655 ?
Ca1A O1A O1A 117.76(15) . 3_655 ?
Ca1 O1A O1A 54.51(12) . 3_655 ?
Ca1 O1A O1A 50.54(8) 3_655 3_655 ?
O2 O1A O1A 91.35(15) 3_655 3_655 ?
O8A O1A O1A 84.00(17) 3_655 3_655 ?
O9 O1A O1A 139.8(2) 3_655 3_655 ?
O1 O1A O1A 79.54(12) 3_655 3_655 ?
Si1 O1A O4A 143.40(16) 3_655 . ?
Ca1A O1A O4A 54.38(11) . . ?
Ca1 O1A O4A 53.76(11) . . ?
Ca1 O1A O4A 122.68(10) 3_655 . ?
O2 O1A O4A 179.08(15) 3_655 . ?
O8A O1A O4A 119.48(16) 3_655 . ?
O9 O1A O4A 117.95(11) 3_655 . ?
O1 O1A O4A 89.62(13) 3_655 . ?
O1A O1A O4A 89.01(15) 3_655 . ?
Si1 O1A OH2A 95.40(14) 3_655 . ?
Ca1A O1A OH2A 46.62(8) . . ?
Ca1 O1A OH2A 104.43(11) . . ?
Ca1 O1A OH2A 144.75(16) 3_655 . ?
O2 O1A OH2A 116.06(14) 3_655 . ?
O8A O1A OH2A 108.79(12) 3_655 . ?
O9 O1A OH2A 62.13(10) 3_655 . ?
O1 O1A OH2A 99.04(16) 3_655 . ?
O1A O1A OH2A 152.59(16) 3_655 . ?
O4A O1A OH2A 63.58(10) . . ?
Si1 O1A OH2 83.59(14) 3_655 . ?
Ca1A O1A OH2 103.79(11) . . ?
Ca1 O1A OH2 45.40(8) . . ?
Ca1 O1A OH2 144.10(16) 3_655 . ?
O2 O1A OH2 117.25(14) 3_655 . ?
O8A O1A OH2 59.60(10) 3_655 . ?
O9 O1A OH2 74.01(10) 3_655 . ?
O1 O1A OH2 151.41(14) 3_655 . ?
O1A O1A OH2 96.99(17) 3_655 . ?
O4A O1A OH2 61.86(10) . . ?
OH2A O1A OH2 71.09(10) . . ?
Si1 O2 Ca4 131.70(19) . . ?
Si1 O2 Ca4A 109.42(19) . . ?
Ca4 O2 Ca4A 106.01(11) . . ?
Si1 O2 Ca1 93.19(13) . . ?
Ca4 O2 Ca1 107.06(13) . . ?
Ca4A O2 Ca1 106.55(13) . . ?
Si1 O2 O1A 35.52(10) . 3_655 ?
Ca4 O2 O1A 127.7(2) . 3_655 ?
Ca4A O2 O1A 126.3(2) . 3_655 ?
Ca1 O2 O1A 59.39(8) . 3_655 ?
Si1 O2 O8A 36.91(11) . . ?
Ca4 O2 O8A 152.92(13) . . ?
Ca4A O2 O8A 72.86(12) . . ?
Ca1 O2 O8A 98.91(13) . . ?
O1A O2 O8A 60.77(12) 3_655 . ?
Si1 O2 O9 32.91(10) . . ?
Ca4 O2 O9 101.74(14) . . ?
Ca4A O2 O9 114.86(14) . . ?
Ca1 O2 O9 119.48(12) . . ?
O1A O2 O9 60.76(10) 3_655 . ?
O8A O2 O9 57.48(11) . . ?
Si1 O2 O4 130.24(17) . . ?
Ca4 O2 O4 54.87(10) . . ?
Ca4A O2 O4 114.09(12) . . ?
Ca1 O2 O4 52.41(8) . . ?
O1A O2 O4 96.93(13) 3_655 . ?
O8A O2 O4 151.23(14) . . ?
O9 O2 O4 130.03(18) . . ?
Si1 O2 O4A 112.74(19) . . ?
Ca4 O2 O4A 114.47(12) . . ?
Ca4A O2 O4A 53.83(10) . . ?
Ca1 O2 O4A 52.92(8) . . ?
O1A O2 O4A 96.52(14) 3_655 . ?
O8A O2 O4A 87.21(15) . . ?
O9 O2 O4A 143.71(17) . . ?
O4 O2 O4A 76.97(10) . . ?
Si1 O2 O3 142.36(15) . 3_656 ?
Ca4 O2 O3 53.08(10) . 3_656 ?
Ca4A O2 O3 53.12(10) . 3_656 ?
Ca1 O2 O3 122.62(10) . 3_656 ?
O1A O2 O3 177.89(13) 3_655 3_656 ?
O8A O2 O3 117.59(16) . 3_656 ?
O9 O2 O3 117.36(11) . 3_656 ?
O4 O2 O3 85.06(12) . 3_656 ?
O4A O2 O3 84.62(12) . 3_656 ?
Si1 O2 OH1 94.94(13) . . ?
Ca4 O2 OH1 45.31(8) . . ?
Ca4A O2 OH1 102.56(10) . . ?
Ca1 O2 OH1 145.10(16) . . ?
O1A O2 OH1 115.71(14) 3_655 . ?
O8A O2 OH1 107.82(12) . . ?
O9 O2 OH1 62.04(10) . . ?
O4 O2 OH1 98.04(15) . . ?
O4A O2 OH1 147.77(12) . . ?
O3 O2 OH1 63.17(10) 3_656 . ?
Si1A O2A Ca4 131.0(2) 1_455 . ?
Si1A O2A Ca4A 108.60(19) 1_455 1_455 ?
Ca4 O2A Ca4A 106.34(11) . 1_455 ?
Si1A O2A Ca1A 93.60(13) 1_455 1_455 ?
Ca4 O2A Ca1A 107.80(13) . 1_455 ?
Ca4A O2A Ca1A 106.94(13) 1_455 1_455 ?
Si1A O2A O1 35.31(9) 1_455 3 ?
Ca4 O2A O1 127.6(2) . 3 ?
Ca4A O2A O1 126.1(2) 1_455 3 ?
Ca1A O2A O1 60.10(8) 1_455 3 ?
Si1A O2A O8A 36.58(11) 1_455 1_455 ?
Ca4 O2A O8A 152.36(13) . 1_455 ?
Ca4A O2A O8A 72.50(12) 1_455 1_455 ?
Ca1A O2A O8A 98.62(12) 1_455 1_455 ?
O1 O2A O8A 60.14(12) 3 1_455 ?
Si1A O2A O9A 33.41(10) 1_455 1_455 ?
Ca4 O2A O9A 100.59(13) . 1_455 ?
Ca4A O2A O9A 113.41(13) 1_455 1_455 ?
Ca1A O2A O9A 120.62(12) 1_455 1_455 ?
O1 O2A O9A 61.15(10) 3 1_455 ?
O8A O2A O9A 57.58(11) 1_455 1_455 ?
Si1A O2A O4 130.86(18) 1_455 . ?
Ca4 O2A O4 55.19(10) . . ?
Ca4A O2A O4 114.73(12) 1_455 . ?
Ca1A O2A O4 52.85(8) 1_455 . ?
O1 O2A O4 97.77(14) 3 . ?
O8A O2A O4 151.36(14) 1_455 . ?
O9A O2A O4 130.54(18) 1_455 . ?
Si1A O2A O4A 112.97(19) 1_455 1_455 ?
Ca4 O2A O4A 115.18(12) . 1_455 ?
Ca4A O2A O4A 53.91(10) 1_455 1_455 ?
Ca1A O2A O4A 53.28(8) 1_455 1_455 ?
O1 O2A O4A 97.34(14) 3 1_455 ?
O8A O2A O4A 87.01(15) 1_455 1_455 ?
O9A O2A O4A 143.99(17) 1_455 1_455 ?
O4 O2A O4A 77.50(10) . 1_455 ?
Si1A O2A O3A 141.84(15) 1_455 3_656 ?
Ca4 O2A O3A 53.27(10) . 3_656 ?
Ca4A O2A O3A 53.17(11) 1_455 3_656 ?
Ca1A O2A O3A 122.64(10) 1_455 3_656 ?
O1 O2A O3A 177.14(13) 3 3_656 ?
O8A O2A O3A 117.69(16) 1_455 3_656 ?
O9A O2A O3A 116.27(11) 1_455 3_656 ?
O4 O2A O3A 84.89(12) . 3_656 ?
O4A O2A O3A 84.25(12) 1_455 3_656 ?
Si1A O2A OH1 93.80(13) 1_455 . ?
Ca4 O2A OH1 45.55(8) . . ?
Ca4A O2A OH1 102.05(10) 1_455 . ?
Ca1A O2A OH1 145.91(16) 1_455 . ?
O1 O2A OH1 114.70(14) 3 . ?
O8A O2A OH1 106.98(12) 1_455 . ?
O9A O2A OH1 60.39(10) 1_455 . ?
O4 O2A OH1 98.67(14) . . ?
O4A O2A OH1 147.93(12) 1_455 . ?
O3A O2A OH1 63.68(9) 3_656 . ?
Si1A O2A OH1A 81.53(13) 1_455 1_455 ?
Ca4 O2A OH1A 101.71(10) . 1_455 ?
Ca4A O2A OH1A 43.99(8) 1_455 1_455 ?
Ca1A O2A OH1A 144.26(16) 1_455 1_455 ?
O1 O2A OH1A 115.05(14) 3 1_455 ?
O8A O2A OH1A 57.54(10) 1_455 1_455 ?
O9A O2A OH1A 71.66(10) 1_455 1_455 ?
O4 O2A OH1A 147.15(12) . 1_455 ?
O4A O2A OH1A 96.02(14) 1_455 1_455 ?
O3A O2A OH1A 62.33(10) 3_656 1_455 ?
OH1 O2A OH1A 69.81(9) . 1_455 ?
C1 O3 O4 31.1(2) . . ?
C1 O3 O5 28.8(2) . . ?
O4 O3 O5 59.90(11) . . ?
C1 O3 Ca4 126.7(3) . 3_656 ?
O4 O3 Ca4 131.3(2) . 3_656 ?
O5 O3 Ca4 111.44(16) . 3_656 ?
C1 O3 Ca4A 124.0(3) . 3_656 ?
O4 O3 Ca4A 130.0(2) . 3_656 ?
O5 O3 Ca4A 110.93(16) . 3_656 ?
Ca4 O3 Ca4A 98.50(11) 3_656 3_656 ?
C1 O3 Ca4 95.9(2) . . ?
O4 O3 Ca4 64.76(9) . . ?
O5 O3 Ca4 124.66(14) . . ?
Ca4 O3 Ca4 104.24(12) 3_656 . ?
Ca4A O3 Ca4 103.71(12) 3_656 . ?
C1 O3 O2 149.0(2) . 3_656 ?
O4 O3 O2 179.9(2) . 3_656 ?
O5 O3 O2 120.21(12) . 3_656 ?
Ca4 O3 O2 48.74(10) 3_656 3_656 ?
Ca4A O3 O2 49.94(10) 3_656 3_656 ?
Ca4 O3 O2 115.14(10) . 3_656 ?
C1 O3 O3A 122.4(3) . 3_656 ?
O4 O3 O3A 100.05(17) . 3_656 ?
O5 O3 O3A 138.6(2) . 3_656 ?
Ca4 O3 O3A 108.53(13) 3_656 3_656 ?
Ca4A O3 O3A 51.98(10) 3_656 3_656 ?
Ca4 O3 O3A 51.73(8) . 3_656 ?
O2 O3 O3A 79.83(12) 3_656 3_656 ?
C1 O3 O3 124.5(3) . 3_656 ?
O4 O3 O3 100.61(18) . 3_656 ?
O5 O3 O3 139.6(2) . 3_656 ?
Ca4 O3 O3 52.63(11) 3_656 3_656 ?
Ca4A O3 O3 108.30(15) 3_656 3_656 ?
Ca4 O3 O3 51.62(8) . 3_656 ?
O2 O3 O3 79.34(13) 3_656 3_656 ?
O3A O3 O3 75.48(12) 3_656 3_656 ?
C1 O3 OH1A 92.2(3) . 3_656 ?
O4 O3 OH1A 117.13(17) . 3_656 ?
O5 O3 OH1A 69.79(12) . 3_656 ?
Ca4 O3 OH1A 99.82(10) 3_656 3_656 ?
Ca4A O3 OH1A 43.93(8) 3_656 3_656 ?
Ca4 O3 OH1A 142.57(17) . 3_656 ?
O2 O3 OH1A 62.92(10) 3_656 3_656 ?
O3A O3 OH1A 93.57(15) 3_656 3_656 ?
O3 O3 OH1A 142.09(15) 3_656 3_656 ?
C1 O3 Ca3 72.7(2) . 3_656 ?
O4 O3 Ca3 103.81(10) . 3_656 ?
O5 O3 Ca3 43.92(8) . 3_656 ?
Ca4 O3 Ca3 83.70(8) 3_656 3_656 ?
Ca4A O3 Ca3 82.90(8) 3_656 3_656 ?
Ca4 O3 Ca3 168.55(11) . 3_656 ?
O2 O3 Ca3 76.29(7) 3_656 3_656 ?
O3A O3 Ca3 134.03(16) 3_656 3_656 ?
O3 O3 Ca3 135.63(18) 3_656 3_656 ?
OH1A O3 Ca3 40.51(7) 3_656 3_656 ?
C1A O3A O4A 31.1(2) . . ?
C1A O3A O5A 28.7(2) . . ?
O4A O3A O5A 59.82(11) . . ?
C1A O3A Ca4 125.7(3) . 3_656 ?
O4A O3A Ca4 130.7(2) . 3_656 ?
O5A O3A Ca4 110.69(16) . 3_656 ?
C1A O3A Ca4A 95.6(2) . . ?
O4A O3A Ca4A 64.42(9) . . ?
O5A O3A Ca4A 124.24(14) . . ?
Ca4 O3A Ca4A 104.91(13) 3_656 . ?
C1A O3A Ca4A 123.8(3) . 3_756 ?
O4A O3A Ca4A 130.6(2) . 3_756 ?
O5A O3A Ca4A 110.12(16) . 3_756 ?
Ca4 O3A Ca4A 98.59(10) 3_656 3_756 ?
Ca4A O3A Ca4A 105.16(12) . 3_756 ?
C1A O3A O3A 122.6(3) . 3_756 ?
O4A O3A O3A 100.44(18) . 3_756 ?
O5A O3A O3A 138.2(2) . 3_756 ?
Ca4 O3A O3A 109.55(15) 3_656 3_756 ?
Ca4A O3A O3A 52.65(8) . 3_756 ?
Ca4A O3A O3A 52.51(11) 3_756 3_756 ?
C1A O3A O2A 148.6(2) . 3_656 ?
O4A O3A O2A 179.3(3) . 3_656 ?
O5A O3A O2A 119.91(12) . 3_656 ?
Ca4 O3A O2A 48.59(10) 3_656 3_656 ?
Ca4A O3A O2A 115.85(10) . 3_656 ?
Ca4A O3A O2A 50.09(10) 3_756 3_656 ?
O3A O3A O2A 80.21(13) 3_756 3_656 ?
C1A O3A O3 123.8(3) . 3_656 ?
O4A O3A O3 100.20(17) . 3_656 ?
O5A O3A O3 138.7(2) . 3_656 ?
Ca4 O3A O3 52.72(11) 3_656 3_656 ?
Ca4A O3A O3 52.19(8) . 3_656 ?
Ca4A O3A O3 109.80(13) 3_756 3_656 ?
O3A O3A O3 77.00(12) 3_756 3_656 ?
O2A O3A O3 79.58(12) 3_656 3_656 ?
C1A O3A OH1A 92.2(3) . 3_756 ?
O4A O3A OH1A 117.65(17) . 3_756 ?
O5A O3A OH1A 69.20(12) . 3_756 ?
Ca4 O3A OH1A 98.42(10) 3_656 3_756 ?
Ca4A O3A OH1A 144.37(16) . 3_756 ?
Ca4A O3A OH1A 44.02(8) 3_756 3_756 ?
O3A O3A OH1A 94.35(17) 3_756 3_756 ?
O2A O3A OH1A 62.59(9) 3_656 3_756 ?
O3 O3A OH1A 142.15(13) 3_656 3_756 ?
C1A O3A Ca3A 72.0(2) . 3_656 ?
O4A O3A Ca3A 103.15(10) . 3_656 ?
O5A O3A Ca3A 43.33(8) . 3_656 ?
Ca4 O3A Ca3A 83.07(8) 3_656 3_656 ?
Ca4A O3A Ca3A 167.57(11) . 3_656 ?
Ca4A O3A Ca3A 82.62(8) 3_756 3_656 ?
O3A O3A Ca3A 134.19(18) 3_756 3_656 ?
O2A O3A Ca3A 76.58(7) 3_656 3_656 ?
O3 O3A Ca3A 134.85(16) 3_656 3_656 ?
OH1A O3A Ca3A 39.85(7) 3_756 3_656 ?
C1 O4 O3 31.5(2) . . ?
C1 O4 O5 28.8(2) . . ?
O3 O4 O5 60.34(11) . . ?
C1 O4 Ca1 128.2(3) . . ?
O3 O4 Ca1 130.2(2) . . ?
O5 O4 Ca1 114.46(17) . . ?
C1 O4 Ca1A 127.5(3) . 1_455 ?
O3 O4 Ca1A 131.2(2) . 1_455 ?
O5 O4 Ca1A 115.16(17) . 1_455 ?
Ca1 O4 Ca1A 97.16(11) . 1_455 ?
C1 O4 Ca4 95.0(2) . . ?
O3 O4 Ca4 63.46(9) . . ?
O5 O4 Ca4 123.79(14) . . ?
Ca1 O4 Ca4 101.02(12) . . ?
Ca1A O4 Ca4 101.07(12) 1_455 . ?
C1 O4 O2A 118.9(3) . . ?
O3 O4 O2A 95.46(16) . . ?
O5 O4 O2A 136.9(2) . . ?
Ca1 O4 O2A 108.31(12) . . ?
Ca1A O4 O2A 52.71(10) 1_455 . ?
Ca4 O4 O2A 48.57(8) . . ?
C1 O4 O2 119.6(3) . . ?
O3 O4 O2 94.99(16) . . ?
O5 O4 O2 136.4(2) . . ?
Ca1 O4 O2 52.60(10) . . ?
Ca1A O4 O2 108.12(12) 1_455 . ?
Ca4 O4 O2 48.61(8) . . ?
O2A O4 O2 75.60(10) . . ?
C1 O4 O1 151.3(2) . . ?
O3 O4 O1 177.14(12) . . ?
O5 O4 O1 122.52(13) . . ?
Ca1 O4 O1 49.43(10) . . ?
Ca1A O4 O1 48.45(10) 1_455 . ?
Ca4 O4 O1 113.69(10) . . ?
O2A O4 O1 82.32(11) . . ?
O2 O4 O1 82.73(12) . . ?
C1 O4 OH2 96.0(3) . . ?
O3 O4 OH2 119.83(18) . . ?
O5 O4 OH2 72.48(12) . . ?
Ca1 O4 OH2 45.31(8) . . ?
Ca1A O4 OH2 100.79(11) 1_455 . ?
Ca4 O4 OH2 141.83(16) . . ?
O2A O4 OH2 144.29(13) . . ?
O2 O4 OH2 94.74(15) . . ?
O1 O4 OH2 62.22(10) . . ?
C1 O4 OH2A 96.1(3) . 1_455 ?
O3 O4 OH2A 121.34(18) . 1_455 ?
O5 O4 OH2A 73.39(12) . 1_455 ?
Ca1 O4 OH2A 99.96(11) . 1_455 ?
Ca1A O4 OH2A 45.24(8) 1_455 1_455 ?
Ca4 O4 OH2A 142.30(16) . 1_455 ?
O2A O4 OH2A 95.01(14) . 1_455 ?
O2 O4 OH2A 143.38(12) . 1_455 ?
O1 O4 OH2A 60.81(10) . 1_455 ?
OH2 O4 OH2A 72.22(10) . 1_455 ?
C1 O4 Ca2A 75.4(2) . 2_655 ?
O3 O4 Ca2A 106.92(10) . 2_655 ?
O5 O4 Ca2A 46.59(9) . 2_655 ?
Ca1 O4 Ca2A 85.14(9) . 2_655 ?
Ca1A O4 Ca2A 85.33(9) 1_455 2_655 ?
Ca4 O4 Ca2A 170.38(11) . 2_655 ?
O2A O4 Ca2A 136.56(15) . 2_655 ?
O2 O4 Ca2A 136.28(15) . 2_655 ?
O1 O4 Ca2A 75.93(7) . 2_655 ?
OH2 O4 Ca2A 41.54(7) . 2_655 ?
OH2A O4 Ca2A 41.55(7) 1_455 2_655 ?
C1A O4A O5A 28.8(2) . . ?
C1A O4A O3A 31.5(2) . . ?
O5A O4A O3A 60.26(11) . . ?
C1A O4A Ca1 127.5(3) . . ?
O5A O4A Ca1 113.63(17) . . ?
O3A O4A Ca1 130.2(2) . . ?
C1A O4A Ca1A 125.7(3) . . ?
O5A O4A Ca1A 113.28(17) . . ?
O3A O4A Ca1A 130.1(2) . . ?
Ca1 O4A Ca1A 98.84(11) . . ?
C1A O4A Ca4A 94.6(2) . . ?
O5A O4A Ca4A 123.33(14) . . ?
O3A O4A Ca4A 63.07(9) . . ?
Ca1 O4A Ca4A 102.18(12) . . ?
Ca1A O4A Ca4A 102.21(12) . . ?
C1A O4A O1A 151.1(2) . . ?
O5A O4A O1A 122.34(13) . . ?
O3A O4A O1A 177.29(14) . . ?
Ca1 O4A O1A 50.33(10) . . ?
Ca1A O4A O1A 48.94(10) . . ?
Ca4A O4A O1A 114.32(10) . . ?
C1A O4A O2A 117.7(3) . 1_655 ?
O5A O4A O2A 135.0(2) . 1_655 ?
O3A O4A O2A 95.10(16) . 1_655 ?
Ca1 O4A O2A 110.93(12) . 1_655 ?
Ca1A O4A O2A 52.36(10) . 1_655 ?
Ca4A O4A O2A 50.07(8) . 1_655 ?
O1A O4A O2A 82.42(12) . 1_655 ?
C1A O4A O2 119.4(3) . . ?
O5A O4A O2 135.7(2) . . ?
O3A O4A O2 95.35(16) . . ?
Ca1 O4A O2 52.41(10) . . ?
Ca1A O4A O2 110.59(12) . . ?
Ca4A O4A O2 49.96(8) . . ?
O1A O4A O2 83.12(12) . . ?
O2A O4A O2 78.87(10) 1_655 . ?
C1A O4A OH2 95.7(3) . . ?
O5A O4A OH2 71.97(12) . . ?
O3A O4A OH2 120.14(17) . . ?
Ca1 O4A OH2 45.39(8) . . ?
Ca1A O4A OH2 99.94(11) . . ?
Ca4A O4A OH2 143.37(16) . . ?
O1A O4A OH2 62.31(10) . . ?
O2A O4A OH2 144.71(13) 1_655 . ?
O2 O4A OH2 94.87(14) . . ?
C1A O4A OH2A 95.3(3) . . ?
O5A O4A OH2A 72.25(12) . . ?
O3A O4A OH2A 120.65(17) . . ?
Ca1 O4A OH2A 99.51(10) . . ?
Ca1A O4A OH2A 45.00(8) . . ?
Ca4A O4A OH2A 143.32(16) . . ?
O1A O4A OH2A 60.82(10) . . ?
O2A O4A OH2A 94.50(14) 1_655 . ?
O2 O4A OH2A 143.92(13) . . ?
OH2 O4A OH2A 70.22(10) . . ?
C1A O4A Ca2 74.4(2) . 2_655 ?
O5A O4A Ca2 45.60(9) . 2_655 ?
O3A O4A Ca2 105.86(10) . 2_655 ?
Ca1 O4A Ca2 85.03(9) . 2_655 ?
Ca1A O4A Ca2 84.74(9) . 2_655 ?
Ca4A O4A Ca2 168.94(11) . 2_655 ?
O1A O4A Ca2 76.74(7) . 2_655 ?
O2A O4A Ca2 135.21(15) 1_655 2_655 ?
O2 O4A Ca2 135.72(15) . 2_655 ?
OH2 O4A Ca2 40.88(7) . 2_655 ?
OH2A O4A Ca2 40.78(7) . 2_655 ?
C1 O5 O4 29.71(17) . . ?
C1 O5 O3 30.08(17) . . ?
O4 O5 O3 59.76(15) . . ?
C1 O5 Ca3 125.8(2) . 3_656 ?
O4 O5 Ca3 155.51(16) . 3_656 ?
O3 O5 Ca3 95.77(11) . 3_656 ?
C1 O5 Ca2A 121.2(2) . 2_655 ?
O4 O5 Ca2A 91.48(11) . 2_655 ?
O3 O5 Ca2A 151.24(15) . 2_655 ?
Ca3 O5 Ca2A 112.98(14) 3_656 2_655 ?
C1 O5 OH1A 93.9(2) . 3_656 ?
O4 O5 OH1A 117.58(16) . 3_656 ?
O3 O5 OH1A 70.50(12) . 3_656 ?
Ca3 O5 OH1A 45.30(8) 3_656 3_656 ?
Ca2A O5 OH1A 130.22(13) 2_655 3_656 ?
C1A O5A O4A 29.86(17) . . ?
C1A O5A O3A 30.08(18) . . ?
O4A O5A O3A 59.92(15) . . ?
C1A O5A Ca3A 126.9(2) . 3_656 ?
O4A O5A Ca3A 156.76(16) . 3_656 ?
O3A O5A Ca3A 96.84(11) . 3_656 ?
C1A O5A Ca2 122.8(2) . 2_655 ?
O4A O5A Ca2 92.95(11) . 2_655 ?
O3A O5A Ca2 152.88(15) . 2_655 ?
Ca3A O5A Ca2 110.28(14) 3_656 2_655 ?
C1A O5A O8 178.0(2) . 2_655 ?
O4A O5A O8 148.29(13) . 2_655 ?
O3A O5A O8 151.79(13) . 2_655 ?
Ca3A O5A O8 54.95(8) 3_656 2_655 ?
Ca2 O5A O8 55.33(8) 2_655 2_655 ?
C1A O5A OH1A 94.9(2) . 3_756 ?
O4A O5A OH1A 119.11(16) . 3_756 ?
O3A O5A OH1A 70.92(12) . 3_756 ?
Ca3A O5A OH1A 45.07(7) 3_656 3_756 ?
Ca2 O5A OH1A 129.31(14) 2_655 3_756 ?
O8 O5A OH1A 86.18(11) 2_655 3_756 ?
C1A O5A OH1 95.9(2) . 3_656 ?
O4A O5A OH1 119.21(16) . 3_656 ?
O3A O5A OH1 70.86(12) . 3_656 ?
Ca3A O5A OH1 44.74(7) 3_656 3_656 ?
Ca2 O5A OH1 129.45(14) 2_655 3_656 ?
O8 O5A OH1 86.10(11) 2_655 3_656 ?
OH1A O5A OH1 69.68(8) 3_756 3_656 ?
C1A O5A OH2 93.1(2) . . ?
O4A O5A OH2 68.24(12) . . ?
O3A O5A OH2 116.90(16) . . ?
Ca3A O5A OH2 129.09(14) 3_656 . ?
Ca2 O5A OH2 44.15(7) 2_655 . ?
O8 O5A OH2 85.82(10) 2_655 . ?
OH1A O5A OH2 171.97(15) 3_756 . ?
OH1 O5A OH2 110.32(11) 3_656 . ?
Si2 O6 Ca2A 137.67(16) . . ?
Si2 O6 Ca3 122.66(15) . . ?
Ca2A O6 Ca3 97.99(10) . . ?
Si2 O6 O8 40.17(10) . . ?
Ca2A O6 O8 137.88(14) . . ?
Ca3 O6 O8 111.02(12) . . ?
Si2 O6 O9 34.83(10) . . ?
Ca2A O6 O9 150.79(15) . . ?
Ca3 O6 O9 91.04(11) . . ?
O8 O6 O9 60.80(11) . . ?
Si2 O6 Ca2 96.39(14) . . ?
Ca2A O6 Ca2 95.46(10) . . ?
Ca3 O6 Ca2 89.04(9) . . ?
O8 O6 Ca2 56.72(9) . . ?
O9 O6 Ca2 112.50(13) . . ?
Si2 O6 O7 29.54(9) . . ?
Ca2A O6 O7 108.14(11) . . ?
Ca3 O6 O7 150.17(12) . . ?
O8 O6 O7 56.99(10) . . ?
O9 O6 O7 59.13(10) . . ?
Ca2 O6 O7 102.20(11) . . ?
Si2 O6 OH2 131.78(15) . 2_645 ?
Ca2A O6 OH2 49.20(8) . 2_645 ?
Ca3 O6 OH2 91.06(10) . 2_645 ?
O8 O6 OH2 98.95(12) . 2_645 ?
O9 O6 OH2 158.86(15) . 2_645 ?
Ca2 O6 OH2 46.52(8) . 2_645 ?
O7 O6 OH2 116.79(11) . 2_645 ?
Si2 O6 O7A 166.03(17) . 4_556 ?
Ca2A O6 O7A 50.26(8) . 4_556 ?
Ca3 O6 O7A 47.74(8) . 4_556 ?
O8 O6 O7A 146.70(15) . 4_556 ?
O9 O6 O7A 131.56(14) . 4_556 ?
Ca2 O6 O7A 93.69(11) . 4_556 ?
O7 O6 O7A 154.80(16) . 4_556 ?
OH2 O6 O7A 62.02(9) 2_645 4_556 ?
Si2 O6 OH1A 108.79(14) . . ?
Ca2A O6 OH1A 89.71(10) . . ?
Ca3 O6 OH1A 46.85(7) . . ?
O8 O6 OH1A 132.41(13) . . ?
O9 O6 OH1A 76.36(11) . . ?
Ca2 O6 OH1A 135.84(11) . . ?
O7 O6 OH1A 117.70(11) . . ?
OH2 O6 OH1A 119.38(11) 2_645 . ?
O7A O6 OH1A 57.36(9) 4_556 . ?
Si2A O6A Ca2A 133.32(16) 1_455 1_455 ?
Si2A O6A Ca3A 123.13(15) 1_455 . ?
Ca2A O6A Ca3A 99.67(11) 1_455 . ?
Si2A O6A O8 40.29(10) 1_455 . ?
Ca2A O6A O8 138.03(14) 1_455 . ?
Ca3A O6A O8 114.09(13) . . ?
Si2A O6A Ca2 97.80(14) 1_455 . ?
Ca2A O6A Ca2 97.92(10) 1_455 . ?
Ca3A O6A Ca2 92.60(10) . . ?
O8 O6A Ca2 58.07(9) . . ?
Si2A O6A O9A 34.89(10) 1_455 1_455 ?
Ca2A O6A O9A 146.23(14) 1_455 1_455 ?
Ca3A O6A O9A 90.39(11) . 1_455 ?
O8 O6A O9A 60.81(11) . 1_455 ?
Ca2 O6A O9A 113.84(13) . 1_455 ?
Si2A O6A O7A 29.38(9) 1_455 1_455 ?
Ca2A O6A O7A 104.02(12) 1_455 1_455 ?
Ca3A O6A O7A 149.07(12) . 1_455 ?
O8 O6A O7A 57.17(10) . 1_455 ?
Ca2 O6A O7A 103.40(11) . 1_455 ?
O9A O6A O7A 59.01(10) 1_455 1_455 ?
Si2A O6A OH2A 133.88(16) 1_455 2_645 ?
Ca2A O6A OH2A 50.48(9) 1_455 2_645 ?
Ca3A O6A OH2A 92.68(10) . 2_645 ?
O8 O6A OH2A 101.75(13) . 2_645 ?
Ca2 O6A OH2A 48.11(8) . 2_645 ?
O9A O6A OH2A 161.79(15) 1_455 2_645 ?
O7A O6A OH2A 117.74(11) 1_455 2_645 ?
Si2A O6A OH1A 105.84(14) 1_455 1_455 ?
Ca2A O6A OH1A 89.70(11) 1_455 1_455 ?
Ca3A O6A OH1A 46.47(7) . 1_455 ?
O8 O6A OH1A 131.56(13) . 1_455 ?
Ca2 O6A OH1A 139.05(11) . 1_455 ?
O9A O6A OH1A 74.08(10) 1_455 1_455 ?
O7A O6A OH1A 113.67(11) 1_455 1_455 ?
OH2A O6A OH1A 120.22(12) 2_645 1_455 ?
Si2 O7 Ca3 132.00(16) . 4 ?
Si2 O7 Ca2 124.68(15) . 4 ?
Ca3 O7 Ca2 99.47(11) 4 4 ?
Si2 O7 O8 40.46(10) . . ?
Ca3 O7 O8 137.25(14) 4 . ?
Ca2 O7 O8 115.06(13) 4 . ?
Si2 O7 Ca3A 97.52(14) . 4 ?
Ca3 O7 Ca3A 98.23(10) 4 4 ?
Ca2 O7 Ca3A 92.72(10) 4 4 ?
O8 O7 Ca3A 57.67(9) . 4 ?
Si2 O7 O9 34.65(9) . . ?
Ca3 O7 O9 145.47(14) 4 . ?
Ca2 O7 O9 92.13(11) 4 . ?
O8 O7 O9 60.75(11) . . ?
Ca3A O7 O9 113.68(13) 4 . ?
Si2 O7 O6 29.35(9) . . ?
Ca3 O7 O6 102.75(11) 4 . ?
Ca2 O7 O6 150.54(12) 4 . ?
O8 O7 O6 57.25(10) . . ?
Ca3A O7 O6 102.91(11) 4 . ?
O9 O7 O6 58.79(10) . . ?
Si2 O7 OH1 132.30(15) . 4 ?
Ca3 O7 OH1 50.47(8) 4 4 ?
Ca2 O7 OH1 93.40(10) 4 4 ?
O8 O7 OH1 100.87(12) . 4 ?
Ca3A O7 OH1 48.27(7) 4 4 ?
O9 O7 OH1 161.35(15) . 4 ?
O6 O7 OH1 115.67(11) . 4 ?
Si2 O7 OH2 107.01(14) . 3_655 ?
Ca3 O7 OH2 89.14(11) 4 3_655 ?
Ca2 O7 OH2 46.49(8) 4 3_655 ?
O8 O7 OH2 132.80(14) . 3_655 ?
Ca3A O7 OH2 139.18(11) 4 3_655 ?
O9 O7 OH2 75.54(11) . 3_655 ?
O6 O7 OH2 114.54(11) . 3_655 ?
OH1 O7 OH2 120.51(11) 4 3_655 ?
Si2A O7A Ca3 136.44(16) . 4 ?
Si2A O7A Ca2A 123.92(15) . 4 ?
Ca3 O7A Ca2A 97.91(10) 4 4 ?
Si2A O7A O8 39.92(10) . 1_655 ?
Ca3 O7A O8 137.63(14) 4 1_655 ?
Ca2A O7A O8 111.96(13) 4 1_655 ?
Si2A O7A O9A 34.61(10) . . ?
Ca3 O7A O9A 149.61(14) 4 . ?
Ca2A O7A O9A 92.58(11) 4 . ?
O8 O7A O9A 60.62(11) 1_655 . ?
Si2A O7A Ca3A 96.02(14) . 4_655 ?
Ca3 O7A Ca3A 96.15(10) 4 4_655 ?
Ca2A O7A Ca3A 89.24(9) 4 4_655 ?
O8 O7A Ca3A 56.64(9) 1_655 4_655 ?
O9A O7A Ca3A 112.50(13) . 4_655 ?
Si2A O7A O6A 29.55(9) . 1_655 ?
Ca3 O7A O6A 106.90(11) 4 1_655 ?
Ca2A O7A O6A 151.41(12) 4 1_655 ?
O8 O7A O6A 56.80(10) 1_655 1_655 ?
O9A O7A O6A 58.84(10) . 1_655 ?
Ca3A O7A O6A 101.75(11) 4_655 1_655 ?
Si2A O7A OH1A 130.53(15) . 4 ?
Ca3 O7A OH1A 49.49(8) 4 4 ?
Ca2A O7A OH1A 91.76(10) 4 4 ?
O8 O7A OH1A 98.62(12) 1_655 4 ?
O9A O7A OH1A 158.83(14) . 4 ?
Ca3A O7A OH1A 46.84(7) 4_655 4 ?
O6A O7A OH1A 115.07(11) 1_655 4 ?
Si2A O7A O6 167.31(17) . 4 ?
Ca3 O7A O6 50.00(8) 4 4 ?
Ca2A O7A O6 47.91(8) 4 4 ?
O8 O7A O6 147.11(14) 1_655 4 ?
O9A O7A O6 133.16(13) . 4 ?
Ca3A O7A O6 93.65(10) 4_655 4 ?
O6A O7A O6 153.94(15) 1_655 4 ?
OH1A O7A O6 62.12(9) 4 4 ?
Si2A O7A OH2 109.82(14) . 3_655 ?
Ca3 O7A OH2 89.15(11) 4 3_655 ?
Ca2A O7A OH2 46.71(7) 4 3_655 ?
O8 O7A OH2 133.20(13) 1_655 3_655 ?
O9A O7A OH2 77.50(11) . 3_655 ?
Ca3A O7A OH2 135.88(11) 4_655 3_655 ?
O6A O7A OH2 118.49(12) 1_655 3_655 ?
OH1A O7A OH2 119.64(11) 4 3_655 ?
O6 O7A OH2 57.53(9) 4 3_655 ?
Si2A O8 Si2 142.00(19) 1_455 . ?
Si2A O8 Ca3A 102.42(12) 1_455 4 ?
Si2 O8 Ca3A 100.68(12) . 4 ?
Si2A O8 Ca2 101.10(12) 1_455 . ?
Si2 O8 Ca2 102.57(12) . . ?
Ca3A O8 Ca2 103.00(11) 4 . ?
Si2A O8 O6A 38.00(9) 1_455 . ?
Si2 O8 O6A 142.95(14) . . ?
Ca3A O8 O6A 115.64(13) 4 . ?
Ca2 O8 O6A 63.67(9) . . ?
Si2A O8 O7 142.23(14) 1_455 . ?
Si2 O8 O7 37.81(9) . . ?
Ca3A O8 O7 63.49(9) 4 . ?
Ca2 O8 O7 115.92(13) . . ?
O6A O8 O7 179.02(16) . . ?
Si2A O8 O7A 37.43(9) 1_455 1_455 ?
Si2 O8 O7A 142.29(14) . 1_455 ?
Ca3A O8 O7A 65.56(9) 4 1_455 ?
Ca2 O8 O7A 114.53(13) . 1_455 ?
O6A O8 O7A 66.03(12) . 1_455 ?
O7 O8 O7A 113.66(12) . 1_455 ?
Si2A O8 O6 143.13(14) 1_455 . ?
Si2 O8 O6 37.29(9) . . ?
Ca3A O8 O6 113.92(13) 4 . ?
Ca2 O8 O6 65.80(9) . . ?
O6A O8 O6 114.55(12) . . ?
O7 O8 O6 65.76(12) . . ?
O7A O8 O6 179.40(14) 1_455 . ?
Si2A O8 O9A 36.95(10) 1_455 1_455 ?
Si2 O8 O9A 105.06(15) . 1_455 ?
Ca3A O8 O9A 122.01(11) 4 1_455 ?
Ca2 O8 O9A 120.18(11) . 1_455 ?
O6A O8 O9A 62.29(11) . 1_455 ?
O7 O8 O9A 118.48(13) . 1_455 ?
O7A O8 O9A 62.28(11) 1_455 1_455 ?
O6 O8 O9A 118.05(14) . 1_455 ?
Si2A O8 O9 105.08(15) 1_455 . ?
Si2 O8 O9 36.92(10) . . ?
Ca3A O8 O9 120.33(11) 4 . ?
Ca2 O8 O9 121.66(11) . . ?
O6A O8 O9 118.67(14) . . ?
O7 O8 O9 62.30(11) . . ?
O7A O8 O9 117.97(14) 1_455 . ?
O6 O8 O9 61.96(11) . . ?
O9A O8 O9 68.14(12) 1_455 . ?
Si2A O8 O5A 109.08(15) 1_455 2_645 ?
Si2 O8 O5A 108.92(15) . 2_645 ?
Ca3A O8 O5A 51.46(7) 4 2_645 ?
Ca2 O8 O5A 51.53(7) . 2_645 ?
O6A O8 O5A 89.50(12) . 2_645 ?
O7 O8 O5A 89.58(12) . 2_645 ?
O7A O8 O5A 90.02(12) 1_455 2_645 ?
O6 O8 O5A 89.84(12) . 2_645 ?
O9A O8 O5A 146.02(15) 1_455 2_645 ?
O9 O8 O5A 145.83(15) . 2_645 ?
Si1 O8A Si1A 155.4(2) . . ?
Si1 O8A O9 37.69(11) . . ?
Si1A O8A O9 166.74(19) . . ?
Si1 O8A O9A 166.98(19) . . ?
Si1A O8A O9A 37.57(10) . . ?
O9 O8A O9A 129.31(16) . . ?
Si1 O8A O2 36.00(10) . . ?
Si1A O8A O2 128.74(16) . . ?
O9 O8A O2 62.95(12) . . ?
O9A O8A O2 149.51(13) . . ?
Si1 O8A O1 127.34(16) . 3_655 ?
Si1A O8A O1 35.17(10) . 3_655 ?
O9 O8A O1 147.85(13) . 3_655 ?
O9A O8A O1 62.53(12) . 3_655 ?
O2 O8A O1 124.85(16) . 3_655 ?
Si1 O8A O2A 128.81(17) . 1_655 ?
Si1A O8A O2A 35.60(10) . 1_655 ?
O9 O8A O2A 151.23(13) . 1_655 ?
O9A O8A O2A 62.25(12) . 1_655 ?
O2 O8A O2A 94.71(12) . 1_655 ?
O1 O8A O2A 59.41(12) 3_655 1_655 ?
Si1 O8A O1A 34.95(10) . 3_655 ?
Si1A O8A O1A 127.26(16) . 3_655 ?
O9 O8A O1A 62.20(12) . 3_655 ?
O9A O8A O1A 149.39(14) . 3_655 ?
O2 O8A O1A 59.51(12) . 3_655 ?
O1 O8A O1A 93.61(12) 3_655 3_655 ?
O2A O8A O1A 123.87(16) 1_655 3_655 ?
Si1 O8A OH1A 96.13(12) . . ?
Si1A O8A OH1A 94.17(12) . . ?
O9 O8A OH1A 83.06(11) . . ?
O9A O8A OH1A 80.21(11) . . ?
O2 O8A OH1A 73.57(10) . . ?
O1 O8A OH1A 128.69(13) 3_655 . ?
O2A O8A OH1A 72.75(10) 1_655 . ?
O1A O8A OH1A 130.20(14) 3_655 . ?
Si1 O8A OH2 92.25(12) . 3_655 ?
Si1A O8A OH2 93.66(12) . 3_655 ?
O9 O8A OH2 80.75(11) . 3_655 ?
O9A O8A OH2 83.19(11) . 3_655 ?
O2 O8A OH2 127.19(14) . 3_655 ?
O1 O8A OH2 70.68(11) 3_655 3_655 ?
O2A O8A OH2 127.97(14) 1_655 3_655 ?
O1A O8A OH2 70.22(10) 3_655 3_655 ?
OH1A O8A OH2 141.11(15) . 3_655 ?
Si1 O8A Ca4A 85.95(11) . . ?
Si1A O8A Ca4A 85.37(11) . . ?
O9 O8A Ca4A 101.58(11) . . ?
O9A O8A Ca4A 99.94(10) . . ?
O2 O8A Ca4A 50.21(9) . . ?
O1 O8A Ca4A 105.28(12) 3_655 . ?
O2A O8A Ca4A 50.12(8) 1_655 . ?
O1A O8A Ca4A 105.05(12) 3_655 . ?
OH1A O8A Ca4A 45.70(7) . . ?
OH2 O8A Ca4A 173.18(13) 3_655 . ?
Si1 O8A Ca1 83.87(10) . 3_655 ?
Si1A O8A Ca1 83.52(10) . 3_655 ?
O9 O8A Ca1 100.48(10) . 3_655 ?
O9A O8A Ca1 101.12(11) . 3_655 ?
O2 O8A Ca1 103.38(11) . 3_655 ?
O1 O8A Ca1 48.47(9) 3_655 3_655 ?
O2A O8A Ca1 102.39(11) 1_655 3_655 ?
O1A O8A Ca1 49.11(9) 3_655 3_655 ?
OH1A O8A Ca1 173.79(13) . 3_655 ?
OH2 O8A Ca1 45.00(7) 3_655 3_655 ?
Ca4A O8A Ca1 128.20(11) . 3_655 ?
Si1 O9 Si2 150.0(2) . . ?
Si1 O9 O8A 38.63(11) . . ?
Si2 O9 O8A 111.42(17) . . ?
Si1 O9 O8 172.05(19) . . ?
Si2 O9 O8 37.92(10) . . ?
O8A O9 O8 149.30(15) . . ?
Si1 O9 O6 128.84(17) . . ?
Si2 O9 O6 33.28(9) . . ?
O8A O9 O6 96.28(13) . . ?
O8 O9 O6 57.24(10) . . ?
Si1 O9 O7 129.22(17) . . ?
Si2 O9 O7 33.33(9) . . ?
O8A O9 O7 98.62(13) . . ?
O8 O9 O7 56.94(10) . . ?
O6 O9 O7 62.07(11) . . ?
Si1 O9 O1A 33.10(10) . 3_655 ?
Si2 O9 O1A 147.50(17) . 3_655 ?
O8A O9 O1A 60.46(12) . 3_655 ?
O8 O9 O1A 142.95(15) . 3_655 ?
O6 O9 O1A 156.37(17) . 3_655 ?
O7 O9 O1A 114.21(13) . 3_655 ?
Si1 O9 O2 32.89(10) . . ?
Si2 O9 O2 149.14(17) . . ?
O8A O9 O2 59.57(12) . . ?
O8 O9 O2 142.60(15) . . ?
O6 O9 O2 115.87(14) . . ?
O7 O9 O2 158.17(17) . . ?
O1A O9 O2 57.93(11) 3_655 . ?
Si1 O9 O9A 116.23(16) . 1_455 ?
Si2 O9 O9A 93.73(14) . 1_455 ?
O8A O9 O9A 154.74(14) . 1_455 ?
O8 O9 O9A 55.82(10) . 1_455 ?
O6 O9 O9A 104.12(12) . 1_455 ?
O7 O9 O9A 104.00(13) . 1_455 ?
O1A O9 O9A 99.40(14) 3_655 1_455 ?
O2 O9 O9A 97.57(14) . 1_455 ?
Si1 O9 OH2A 100.29(14) . 3_655 ?
Si2 O9 OH2A 93.16(13) . 3_655 ?
O8A O9 OH2A 115.33(13) . 3_655 ?
O8 O9 OH2A 76.52(11) . 3_655 ?
O6 O9 OH2A 126.21(13) . 3_655 ?
O7 O9 OH2A 70.63(10) . 3_655 ?
O1A O9 OH2A 67.19(11) 3_655 3_655 ?
O2 O9 OH2A 117.57(13) . 3_655 ?
O9A O9 OH2A 63.38(11) 1_455 3_655 ?
Si1 O9 OH1 100.72(14) . . ?
Si2 O9 OH1 93.96(13) . . ?
O8A O9 OH1 114.05(12) . . ?
O8 O9 OH1 75.53(10) . . ?
O6 O9 OH1 73.05(11) . . ?
O7 O9 OH1 126.68(13) . . ?
O1A O9 OH1 118.35(13) 3_655 . ?
O2 O9 OH1 67.84(11) . . ?
O9A O9 OH1 59.77(10) 1_455 . ?
OH2A O9 OH1 123.01(12) 3_655 . ?
Si1 O9 Ca3 102.05(13) . . ?
Si2 O9 Ca3 73.28(11) . . ?
O8A O9 Ca3 90.09(10) . . ?
O8 O9 Ca3 79.68(9) . . ?
O6 O9 Ca3 41.76(7) . . ?
O7 O9 Ca3 103.83(10) . . ?
O1A O9 Ca3 134.06(11) 3_655 . ?
O2 O9 Ca3 77.15(9) . . ?
O9A O9 Ca3 95.24(10) 1_455 . ?
OH2A O9 Ca3 154.37(12) 3_655 . ?
OH1 O9 Ca3 39.82(7) . . ?
Si1A O9A Si2A 150.3(2) . . ?
Si1A O9A O8A 38.67(11) . . ?
Si2A O9A O8A 111.80(16) . . ?
Si1A O9A O8 171.06(18) . 1_655 ?
Si2A O9A O8 37.66(10) . 1_655 ?
O8A O9A O8 149.41(16) . 1_655 ?
Si1A O9A O6A 131.73(17) . 1_655 ?
Si2A O9A O6A 33.61(9) . 1_655 ?
O8A O9A O6A 98.99(13) . 1_655 ?
O8 O9A O6A 56.90(10) 1_655 1_655 ?
Si1A O9A O7A 126.76(17) . . ?
Si2A O9A O7A 33.16(9) . . ?
O8A O9A O7A 96.36(13) . . ?
O8 O9A O7A 57.10(10) 1_655 . ?
O6A O9A O7A 62.15(11) 1_655 . ?
Si1A O9A O2A 33.45(10) . 1_655 ?
Si2A O9A O2A 151.45(17) . 1_655 ?
O8A O9A O2A 60.17(12) . 1_655 ?
O8 O9A O2A 144.93(15) 1_655 1_655 ?
O6A O9A O2A 117.92(13) 1_655 1_655 ?
O7A O9A O2A 156.54(16) . 1_655 ?
Si1A O9A O1 32.53(10) . 3_655 ?
Si2A O9A O1 145.47(17) . 3_655 ?
O8A O9A O1 59.88(12) . 3_655 ?
O8 O9A O1 140.21(14) 1_655 3_655 ?
O6A O9A O1 158.34(17) 1_655 3_655 ?
O7A O9A O1 112.32(13) . 3_655 ?
O2A O9A O1 57.96(11) 1_655 3_655 ?
Si1A O9A O9 115.68(15) . 1_655 ?
Si2A O9A O9 93.69(14) . 1_655 ?
O8A O9A O9 154.32(14) . 1_655 ?
O8 O9A O9 56.04(10) 1_655 1_655 ?
O6A O9A O9 104.31(13) 1_655 1_655 ?
O7A O9A O9 103.94(13) . 1_655 ?
O2A O9A O9 98.71(13) 1_655 1_655 ?
O1 O9A O9 97.35(13) 3_655 1_655 ?
Si1A O9A OH1 102.47(15) . 1_655 ?
Si2A O9A OH1 94.66(14) . 1_655 ?
O8A O9A OH1 115.89(13) . 1_655 ?
O8 O9A OH1 77.17(11) 1_655 1_655 ?
O6A O9A OH1 72.28(11) 1_655 1_655 ?
O7A O9A OH1 127.51(13) . 1_655 ?
O2A O9A OH1 69.01(11) 1_655 1_655 ?
O1 O9A OH1 119.47(14) 3_655 1_655 ?
O9 O9A OH1 62.71(10) 1_655 1_655 ?
Si1A O9A OH2A 98.24(14) . 3_755 ?
Si2A O9A OH2A 92.48(13) . 3_755 ?
O8A O9A OH2A 113.53(12) . 3_755 ?
O8 O9A OH2A 74.93(10) 1_655 3_755 ?
O6A O9A OH2A 125.59(13) 1_655 3_755 ?
O7A O9A OH2A 71.56(11) . 3_755 ?
O2A O9A OH2A 115.99(13) 1_655 3_755 ?
O1 O9A OH2A 65.71(11) 3_655 3_755 ?
O9 O9A OH2A 60.14(10) 1_655 3_755 ?
OH1 O9A OH2A 122.72(12) 1_655 3_755 ?
Si1A O9A Ca3A 104.21(13) . 1_655 ?
Si2A O9A Ca3A 74.04(10) . 1_655 ?
O8A O9A Ca3A 91.97(10) . 1_655 ?
O8 O9A Ca3A 81.36(9) 1_655 1_655 ?
O6A O9A Ca3A 41.62(7) 1_655 1_655 ?
O7A O9A Ca3A 103.65(10) . 1_655 ?
O2A O9A Ca3A 78.77(9) 1_655 1_655 ?
O1 O9A Ca3A 135.68(12) 3_655 1_655 ?
O9 O9A Ca3A 98.25(10) 1_655 1_655 ?
OH1 O9A Ca3A 40.00(7) 1_655 1_655 ?
OH2A O9A Ca3A 154.29(11) 3_755 1_655 ?
Ca4 OH1 Ca3A 119.65(13) . . ?
Ca4 OH1 Ca3 118.75(13) . . ?
Ca3A OH1 Ca3 108.78(12) . . ?
Ca4 OH1 O7 153.64(11) . 4_556 ?
Ca3A OH1 O7 58.32(9) . 4_556 ?
Ca3 OH1 O7 51.08(9) . 4_556 ?
Ca4 OH1 O9A 91.87(10) . 1_455 ?
Ca3A OH1 O9A 83.27(11) . 1_455 ?
Ca3 OH1 O9A 130.51(12) . 1_455 ?
O7 OH1 O9A 112.99(12) 4_556 1_455 ?
Ca4 OH1 O9 91.30(10) . . ?
Ca3A OH1 O9 131.50(12) . . ?
Ca3 OH1 O9 82.23(10) . . ?
O7 OH1 O9 109.05(12) 4_556 . ?
O9A OH1 O9 57.52(10) 1_455 . ?
Ca4 OH1 O2A 45.95(8) . . ?
Ca3A OH1 O2A 91.57(11) . . ?
Ca3 OH1 O2A 159.63(14) . . ?
O7 OH1 O2A 149.04(14) 4_556 . ?
O9A OH1 O2A 50.59(9) 1_455 . ?
O9 OH1 O2A 84.67(10) . . ?
Ca4 OH1 O2 45.96(8) . . ?
Ca3A OH1 O2 161.21(14) . . ?
Ca3 OH1 O2 89.98(11) . . ?
O7 OH1 O2 140.36(13) 4_556 . ?
O9A OH1 O2 85.18(10) 1_455 . ?
O9 OH1 O2 50.12(8) . . ?
O2A OH1 O2 69.65(9) . . ?
Ca4 OH1 O5A 85.74(10) . 3_656 ?
Ca3A OH1 O5A 46.40(7) . 3_656 ?
Ca3 OH1 O5A 104.51(10) . 3_656 ?
O7 OH1 O5A 75.62(10) 4_556 3_656 ?
O9A OH1 O5A 116.44(12) 1_455 3_656 ?
O9 OH1 O5A 173.25(13) . 3_656 ?
O2A OH1 O5A 88.93(11) . 3_656 ?
O2 OH1 O5A 129.11(12) . 3_656 ?
Ca4 OH1 H1 99.8 . . ?
Ca3A OH1 H1 105.7 . . ?
Ca3 OH1 H1 100.9 . . ?
O7 OH1 H1 106.0 4_556 . ?
O9A OH1 H1 32.0 1_455 . ?
O9 OH1 H1 27.6 . . ?
O2A OH1 H1 73.2 . . ?
O2 OH1 H1 70.4 . . ?
O5A OH1 H1 147.4 3_656 . ?
Ca4A OH1A Ca3A 121.11(13) . 1_655 ?
Ca4A OH1A Ca3 119.47(13) . . ?
Ca3A OH1A Ca3 109.09(12) 1_655 . ?
Ca4A OH1A O8A 68.75(9) . . ?
Ca3A OH1A O8A 117.93(12) 1_655 . ?
Ca3 OH1A O8A 115.51(12) . . ?
Ca4A OH1A O7A 154.10(11) . 4_556 ?
Ca3A OH1A O7A 59.66(9) 1_655 4_556 ?
Ca3 OH1A O7A 49.66(8) . 4_556 ?
O8A OH1A O7A 136.08(13) . 4_556 ?
Ca4A OH1A O6A 137.01(12) . 1_655 ?
Ca3A OH1A O6A 48.59(8) 1_655 1_655 ?
Ca3 OH1A O6A 100.94(12) . 1_655 ?
O8A OH1A O6A 81.60(10) . 1_655 ?
O7A OH1A O6A 65.50(10) 4_556 1_655 ?
Ca4A OH1A O6 134.97(12) . . ?
Ca3A OH1A O6 101.44(12) 1_655 . ?
Ca3 OH1A O6 49.21(8) . . ?
O8A OH1A O6 79.27(10) . . ?
O7A OH1A O6 60.52(10) 4_556 . ?
O6A OH1A O6 63.02(9) 1_655 . ?
Ca4A OH1A O5A 87.18(11) . 3_756 ?
Ca3A OH1A O5A 47.24(7) 1_655 3_756 ?
Ca3 OH1A O5A 105.92(10) . 3_756 ?
O8A OH1A O5A 138.27(13) . 3_756 ?
O7A OH1A O5A 76.10(10) 4_556 3_756 ?
O6A OH1A O5A 95.81(11) 1_655 3_756 ?
O6 OH1A O5A 136.32(13) . 3_756 ?
Ca4A OH1A O5 87.18(11) . 3_656 ?
Ca3A OH1A O5 104.97(10) 1_655 3_656 ?
Ca3 OH1A O5 46.83(7) . 3_656 ?
O8A OH1A O5 136.98(13) . 3_656 ?
O7A OH1A O5 68.88(10) 4_556 3_656 ?
O6A OH1A O5 134.34(12) 1_655 3_656 ?
O6 OH1A O5 96.03(11) . 3_656 ?
O5A OH1A O5 71.17(8) 3_756 3_656 ?
Ca4A OH1A O3A 49.46(8) . 3_756 ?
Ca3A OH1A O3A 74.05(10) 1_655 3_756 ?
Ca3 OH1A O3A 131.38(11) . 3_756 ?
O8A OH1A O3A 103.15(12) . 3_756 ?
O7A OH1A O3A 115.93(10) 4_556 3_756 ?
O6A OH1A O3A 113.31(12) 1_655 3_756 ?
O6 OH1A O3A 175.47(13) . 3_756 ?
O5A OH1A O3A 39.88(8) 3_756 3_756 ?
O5 OH1A O3A 84.83(10) 3_656 3_756 ?
Ca4A OH1A O3 49.41(8) . 3_656 ?
Ca3A OH1A O3 130.91(11) 1_655 3_656 ?
Ca3 OH1A O3 72.95(10) . 3_656 ?
O8A OH1A O3 102.67(12) . 3_656 ?
O7A OH1A O3 108.38(11) 4_556 3_656 ?
O6A OH1A O3 173.58(13) 1_655 3_656 ?
O6 OH1A O3 112.74(12) . 3_656 ?
O5A OH1A O3 84.22(10) 3_756 3_656 ?
O5 OH1A O3 39.70(8) 3_656 3_656 ?
O3A OH1A O3 70.66(9) 3_756 3_656 ?
Ca4A OH1A O2A 46.70(8) . 1_655 ?
Ca3A OH1A O2A 90.63(11) 1_655 1_655 ?
Ca3 OH1A O2A 160.16(13) . 1_655 ?
O8A OH1A O2A 49.71(9) . 1_655 ?
O7A OH1A O2A 149.52(13) 4_556 1_655 ?
O6A OH1A O2A 90.39(10) 1_655 1_655 ?
O6 OH1A O2A 126.24(10) . 1_655 ?
O5A OH1A O2A 88.87(11) 3_756 1_655 ?
O5 OH1A O2A 131.23(13) 3_656 1_655 ?
O3A OH1A O2A 55.08(9) 3_756 1_655 ?
O3 OH1A O2A 96.03(12) 3_656 1_655 ?
Ca4A OH1A H1A 99.5 . . ?
Ca3A OH1A H1A 103.4 1_655 . ?
Ca3 OH1A H1A 99.5 . . ?
O8A OH1A H1A 30.8 . . ?
O7A OH1A H1A 105.4 4_556 . ?
O6A OH1A H1A 57.1 1_655 . ?
O6 OH1A H1A 53.3 . . ?
O5A OH1A H1A 146.1 3_756 . ?
O5 OH1A H1A 141.8 3_656 . ?
O3A OH1A H1A 127.7 3_756 . ?
O3 OH1A H1A 125.1 3_656 . ?
O2A OH1A H1A 72.9 1_655 . ?
Ca2 OH2 Ca1 121.09(14) 2_655 . ?
Ca2 OH2 Ca2A 109.58(12) 2_655 2_655 ?
Ca1 OH2 Ca2A 118.45(14) . 2_655 ?
Ca2 OH2 O8A 117.60(13) 2_655 3_655 ?
Ca1 OH2 O8A 69.66(9) . 3_655 ?
Ca2A OH2 O8A 115.53(13) 2_655 3_655 ?
Ca2 OH2 O6 60.13(9) 2_655 2_655 ?
Ca1 OH2 O6 153.81(12) . 2_655 ?
Ca2A OH2 O6 49.78(8) 2_655 2_655 ?
O8A OH2 O6 135.30(13) 3_655 2_655 ?
Ca2 OH2 O7 48.95(8) 2_655 3_655 ?
Ca1 OH2 O7 137.20(13) . 3_655 ?
Ca2A OH2 O7 101.79(12) 2_655 3_655 ?
O8A OH2 O7 80.73(10) 3_655 3_655 ?
O6 OH2 O7 65.85(10) 2_655 3_655 ?
Ca2 OH2 O7A 102.15(12) 2_655 3_655 ?
Ca1 OH2 O7A 134.52(13) . 3_655 ?
Ca2A OH2 O7A 49.53(8) 2_655 3_655 ?
O8A OH2 O7A 78.73(10) 3_655 3_655 ?
O6 OH2 O7A 60.46(10) 2_655 3_655 ?
O7 OH2 O7A 63.54(9) 3_655 3_655 ?
Ca2 OH2 O4A 72.54(10) 2_655 . ?
Ca1 OH2 O4A 50.87(9) . . ?
Ca2A OH2 O4A 130.64(12) 2_655 . ?
O8A OH2 O4A 104.53(12) 3_655 . ?
O6 OH2 O4A 114.99(11) 2_655 . ?
O7 OH2 O4A 112.40(13) 3_655 . ?
O7A OH2 O4A 174.58(13) 3_655 . ?
Ca2 OH2 O4 130.06(12) 2_655 . ?
Ca1 OH2 O4 50.13(8) . . ?
Ca2A OH2 O4 71.35(10) 2_655 . ?
O8A OH2 O4 104.39(12) 3_655 . ?
O6 OH2 O4 107.05(11) 2_655 . ?
O7 OH2 O4 172.67(13) 3_655 . ?
O7A OH2 O4 111.89(13) 3_655 . ?
O4A OH2 O4 71.74(10) . . ?
Ca2 OH2 O1A 89.87(12) 2_655 . ?
Ca1 OH2 O1A 47.77(8) . . ?
Ca2A OH2 O1A 160.47(14) 2_655 . ?
O8A OH2 O1A 50.17(9) 3_655 . ?
O6 OH2 O1A 149.11(14) 2_655 . ?
O7 OH2 O1A 89.53(11) 3_655 . ?
O7A OH2 O1A 126.20(11) 3_655 . ?
O4A OH2 O1A 55.84(10) . . ?
O4 OH2 O1A 97.78(12) . . ?
Ca2 OH2 O1 162.46(14) 2_655 . ?
Ca1 OH2 O1 46.79(8) . . ?
Ca2A OH2 O1 87.88(12) 2_655 . ?
O8A OH2 O1 49.73(9) 3_655 . ?
O6 OH2 O1 136.97(14) 2_655 . ?
O7 OH2 O1 127.57(11) 3_655 . ?
O7A OH2 O1 87.81(10) 3_655 . ?
O4A OH2 O1 97.60(12) . . ?
O4 OH2 O1 56.02(10) . . ?
O1A OH2 O1 72.63(10) . . ?
Ca2 OH2 O5A 46.59(8) 2_655 . ?
Ca1 OH2 O5A 88.19(11) . . ?
Ca2A OH2 O5A 104.74(10) 2_655 . ?
O8A OH2 O5A 139.51(13) 3_655 . ?
O6 OH2 O5A 75.23(10) 2_655 . ?
O7 OH2 O5A 95.53(11) 3_655 . ?
O7A OH2 O5A 135.45(12) 3_655 . ?
O4A OH2 O5A 39.78(8) . . ?
O4 OH2 O5A 83.99(11) . . ?
O1A OH2 O5A 89.73(11) . . ?
O1 OH2 O5A 131.94(13) . . ?
Ca2 OH2 H2 104.2 2_655 . ?
Ca1 OH2 H2 101.7 . . ?
Ca2A OH2 H2 97.1 2_655 . ?
O8A OH2 H2 32.3 3_655 . ?
O6 OH2 H2 103.1 2_655 . ?
O7 OH2 H2 56.9 3_655 . ?
O7A OH2 H2 50.5 3_655 . ?
O4A OH2 H2 131.2 . . ?
O4 OH2 H2 125.5 . . ?
O1A OH2 H2 75.7 . . ?
O1 OH2 H2 70.9 . . ?
O5A OH2 H2 148.1 . . ?
Ca2 OH2A Ca1A 119.34(14) 2_655 . ?
Ca2 OH2A Ca2A 109.31(12) 2_655 2_755 ?
Ca1A OH2A Ca2A 117.56(14) . 2_755 ?
Ca2 OH2A O6A 58.89(9) 2_655 2_655 ?
Ca1A OH2A O6A 153.09(12) . 2_655 ?
Ca2A OH2A O6A 51.22(9) 2_755 2_655 ?
Ca2 OH2A O9 84.27(11) 2_655 3_655 ?
Ca1A OH2A O9 92.22(11) . 3_655 ?
Ca2A OH2A O9 130.73(13) 2_755 3_655 ?
O6A OH2A O9 113.45(12) 2_655 3_655 ?
Ca2 OH2A O9A 131.79(12) 2_655 3_755 ?
Ca1A OH2A O9A 91.47(11) . 3_755 ?
Ca2A OH2A O9A 82.83(11) 2_755 3_755 ?
O6A OH2A O9A 109.04(12) 2_655 3_755 ?
O9 OH2A O9A 56.48(10) 3_655 3_755 ?
Ca2 OH2A O1A 90.54(12) 2_655 . ?
Ca1A OH2A O1A 46.96(8) . . ?
Ca2A OH2A O1A 160.09(14) 2_755 . ?
O6A OH2A O1A 148.55(14) 2_655 . ?
O9 OH2A O1A 50.68(9) 3_655 . ?
O9A OH2A O1A 85.06(10) 3_755 . ?
Ca2 OH2A O1 161.88(15) 2_655 1_655 ?
Ca1A OH2A O1 46.55(8) . 1_655 ?
Ca2A OH2A O1 88.74(12) 2_755 1_655 ?
O6A OH2A O1 139.18(14) 2_655 1_655 ?
O9 OH2A O1 85.08(11) 3_655 1_655 ?
O9A OH2A O1 50.03(9) 3_755 1_655 ?
O1A OH2A O1 71.38(10) . 1_655 ?
Ca2 OH2A O4 127.48(11) 2_655 1_655 ?
Ca1A OH2A O4 49.63(8) . 1_655 ?
Ca2A OH2A O4 70.46(10) 2_755 1_655 ?
O6A OH2A O4 107.73(11) 2_655 1_655 ?
O9 OH2A O4 137.51(12) 3_655 1_655 ?
O9A OH2A O4 100.70(12) 3_755 1_655 ?
O1A OH2A O4 96.49(12) . 1_655 ?
O1 OH2A O4 56.07(10) 1_655 1_655 ?
Ca2 OH2A O4A 71.19(10) 2_655 . ?
Ca1A OH2A O4A 50.05(8) . . ?
Ca2A OH2A O4A 128.45(11) 2_755 . ?
O6A OH2A O4A 113.76(11) 2_655 . ?
O9 OH2A O4A 100.82(12) 3_655 . ?
O9A OH2A O4A 136.96(12) 3_755 . ?
O1A OH2A O4A 55.60(10) . . ?
O1 OH2A O4A 96.55(12) 1_655 . ?
O4 OH2A O4A 70.70(9) 1_655 . ?
Ca2 OH2A H2A 107.7 2_655 . ?
Ca1A OH2A H2A 96.7 . . ?
Ca2A OH2A H2A 103.6 2_755 . ?
O6A OH2A H2A 109.5 2_655 . ?
O9 OH2A H2A 30.2 3_655 . ?
O9A OH2A H2A 27.0 3_755 . ?
O1A OH2A H2A 70.5 . . ?
O1 OH2A H2A 68.1 1_655 . ?
O4 OH2A H2A 123.7 1_655 . ?
O4A OH2A H2A 126.0 . . ?
 
_diffrn_measured_fraction_theta_max    0.955
_diffrn_reflns_theta_full              30.01
_diffrn_measured_fraction_theta_full   0.955
_refine_diff_density_max    0.452
_refine_diff_density_min   -0.560
_refine_diff_density_rms    0.096
